«Introduction to the physical material science» This manual is dedicated for the study of regularities and mechanisms of
197 38 4MB
English Pages  Year 2015
В первых главах книги рассмотрены фундаментальные физические и химические положения, непосредственно относящиеся к матер
185 48 11MB Read more
This accessible introductory text explores the history, philosophies, and principles of today's physical education
1,752 41 12MB Read more
Succeed in your non-science majors course with this easy-to-understand text that presents the fundamental concepts of th
996 223 75MB Read more
Consistent with previous editions of AN INTRODUCTION TO PHYSICAL SCIENCE, the goal of the new Fourteenth Edition is to s
707 65 157MB Read more
The manual contains the most important the theoretical information on the discipline «physical culture and sport», by th
234 46 19MB Read more
AL-FARABI KAZAKH NATIONAL UNIVERSITY
O.Yu. Prikhodko, G.A. Ismailova
INTRODUCTION TO THE PHYSICAL MATERIAL SCIENCE Education manual
university Press» 2015
UDC 620 BBC 30.3 Р 92 Recommended to print the scientific session of the physicotechnical faculty of Al-Farabi Kazakh national university and editorial -printing session Reviewers: doctor of physical and mathematical sciences, professor N.E. Korobova PhD, senior lecturer I.E. Berezovskaya
Prikhodko O.Yu., Ismailova G.A. Р 92 Introduction to the physical material science: Education manual / O.Yu. Prikhodko, G.A. Ismailova. – Almaty: Қазақ университеті, 2015. – 187 с. ISBN 978-601-04-1650-5 «Introduction to the physical material science» This manual is dedicated for the study of regularities and mechanisms of materials phase formation in equilibrium and non-equilibrium conditions, dependence of their properties from the ways of creating materials with desired properties. In the manual also describes the main physical properties of metals, semiconductors and dielectrics, features of chemical bondings in the material.
© Prikhodko O.Yu., Ismailova G.A., 2015 © Al-Farabi KazNU, 2015
Foreword ................................................................................................5 INTRODUCTION. TASKS OF THE COURSE «INTRODUCTION TO THE PHYSICAL MATERIAL SCIENCE» ...7 Chapter 1. GENERAL PHYSICAL PROPERTIES OF SEMICONDUCTORS, DIELECTRICS AND METALS .................10 § 1. General provisions ...............................................................10 § 2. Electrical properties .............................................................11 § 3. Optical properties ................................................................35 § 4. Acoustic properties ..............................................................39 § 5. Magnetic properties .............................................................43 § 6. Thermal properties ...............................................................53 § 7. Mechanical properties .........................................................59 Chapter 2. CHEMICAL BONDINGS................................................67 § 1. The structure of atoms and chemical bonding .....................67 § 2. The types of chemical bondings ...........................................72 § 3. Chemical bonding and atomic and ionic radii .....................79 § 4. Features of chemical bondings in metals and semiconductors ...........................................................................82 Chapter 3. PHASE EQUILIBRIUM IN SEMICONDUCTOR, DIELECTRIC AND METAL SYSTEMS .........................................98 § 1. Main aspects of the thermodynamics of phase equilibrium 98 § 2. Phase equilibrium. The rule of phase. Gibbs Law ...............104 § 3. Construction methods of phase equilibrium diagrams .........109 § 4. T – X diagrams of phase equilibrium of binary systems with unlimited solubility of the components ......................................115 § 5. Construction and analysis of diagrams with unlimited solubility according to the data about change of the thermodynamic potential. Coefficient of distribution..................123
§ 6. T – X – diagrams of phase equilibrium of binary systems with unlimited solubility of the components ..............................137 § 7. Dual semiconductor and dielectric phases ...........................154 § 8. Deviations from equilibrium state. The phase equilibrium diagrams role in selecting the conditions of crystallization and thermal treatment ......................................................................... 159 § 9. P – T and P – T – X diagrams of phase equilibrium ............125 Checklist and tasks …………………………………..……... ...............166 LITERATURE........................................................................................176 ATTACHMENT. PHASE DIAGRAMS OF SOME SEMICONDUCTOR SYSTEMS ..........................................................180
The progress of human civilization connected with the progress in development, obtaining and using of different materials. New materials enhanced the work efficiency. Today special significance acquired materials and devices, which designed to increase the effectiveness of mental labor, to ensure progress in computer technology, methods of storage and transmission of information, automation of industry, efficiency conversion of various types of energy with high efficiency PEC. Physical material science – is a scientific discipline that studies the laws and the atomic mechanism of material’s phase formation (metals, semiconductors, dielectrics, etc.) in equilibrium and nonequilibrium conditions, the dependence of bulk and surface properties of these materials on the nature of chemical bonding, chemical and phase composition, structural imperfections and ways of creating materials with desired properties and management of the latter by the action to the chemical composition, phase and structural state of the material. The aim of course is the study of regularities and mechanism of material’s phase formation (metals, semiconductors, dielectrics, etc.) in equilibrium and non- equilibrium conditions, depending on their properties to the nature of chemical bonding, chemical and phase composition and ways of creating materials with desired properties. Important information about the phase composition of alloys in equilibrium and similar conditions, about beginning temperatures and end of phase transformations can be obtained from state diagrams. The state diagrams of binary and ternary systems in combination with the composition-property diagrams are the basis of the doping theory and the creation of alloys with desired properties.
For materials scientists and specialists in related fields state diagrams – is a base for new searching and improvement of existing materials. For metallurgists state diagrams are the basis for the development and improvement of metallurgical processes of obtaining metals and compounds, also their purification from impurities.
INTRODUCTION. TASKS OF THE COURSE «INTRODUCTION TO THE PHYSICAL MATERIAL SCIENCE» Development of materials with desired properties requires a clear understanding of what factors depend these properties and how, and how at least they can be controlled. The properties of materials depended on many factors and determined, at first, by the nature of chemical bonding; phase state of materials; type, concentration and nature of the impurities. Very strong influence on the properties of the materials have defects in the atomic structure, their interaction with each other and with impurities. Historically, existed two approaches about interpretation of the properties and phenomena occurred in solids, particularly in metals: – macroscopic or phenomenological; – microscopic or atomistic. For the macroscopic approach is typical solid interpretation as a continuum without detailing its internal structure. The approach connected with the resistance of materials and other sciences. In the microscopic approach description and explanation of the properties of solids based on the laws of its constituent particle’s interaction, i.e. at the atomic level. In this approach, realized following chain: structure – property. Today microscopic approach is the only strictly scientific approach to the interpretation of the observed properties and phenomena in solids. In general case, for obtaining materials with desired properties it was necessary provide implementation of the following logical sequence: Technology → atomic structure → (energy spectrum) → physicochemical properties → technology The object of study in material science are high degree purified single crystals of semiconductors, which not found in nature, i.e. processed materials. The theoretical foundations of physical material science include: – periodic law of Mendeleev – laws of thermodynamics,
– theory of chemical bonding, – band theory of solids, – position about the role of short-range order in the arrangement of atoms in formation of the semiconductors and dielectrics properties (was formulated at first by A.F. Ioffe). Material science originated in the middle of 19th century. Leading scientists, who was initiating material science – is Anosov (1797-1831 yy.) and Chernov (1839-1921 yy.). Formation of semiconductor material science started in the 3040 years of 20th century under the direction of academician A.F. Ioffe. In the 20 years in the USA developed ferroelectric properties of Rochelle salt. In 1944, in the USSR academician Wool developed ferroelectric properties of barium titanate (BaTi). In 1948–1949 yy. in the USA Bardeen, Shockley and Brayteyn – created the first transistor. In the early 40-ies the USA launched the first atomic reactor. In 1950– Till and Little obtained the first single crystal of germanium with instrument impurity. In 1958 in the USA and USSR was marked by obtaining dislocation-free silicon. In 1955–1960 yy. – development of space technology, which required the creation of new materials. 1960 years- USSR – the creation of the first solid-state laser generator on gallium arsenide (GaAs) (Basov, Nasledov, Rivkin). 1950 years USSR – development of chalcogenide vitreous semiconductors – CVS (Kolomiets, Goryunova). 1975 year- USA- were first obtained films of amorphous silicon (a-Si), and later the films of amorphous hydrogenated silicon (a-Si: H), (Speer, Le Comber). 1960-1970 yy. – the creation of theory and technology of heterostructures. (Zh.I. Alferov) 1970 yy. – the creation of VLIS – very large integrated microcircuits. 1980 yy. – the creation of extralattices (superlattices). 1990 yy. -opening of quantum size effects in solid, which was the beginning of the creation of lasers based on quantum wells and quantum dots. 8
Nowadays provide intensive research of new materials and developing new technologies and devices: composites, polymers, amorphous metals; powder metallurgy, radiation technology, hightemperature superconductivity; construction materials; fullerenes, nanotubes, nanowires; developed tools to nanomaterials. In Figure 1.1. showed the position of materials science in the general structure of science.
Figure 1.1.– The position of materials science in the general structure of science
The main tasks of the course "Introduction to the physical material science" is establishment of the relationship between the composition, structure and properties of materials, the study of thermal, chemical and thermal treatment and other methods of hardening, the formation of knowledge about the properties of the main types of materials and their application field.
GENERAL PHYSICAL PROPERTIES OF SEMICONDUCTORS, DIELECTRICS AND METALS
§ 1. General provisions The basic physical properties of semiconductors, dielectrics and metals, advisable to consider in order to facilitate understanding of the influence regularities to the properties of the material composition and obtaining technology. Material properties of practical interest is very diverse, so we consider the properties of the most important materials used in semiconductor electronics. This group of properties we can classified as following: Table 1.1. The basic physical properties of semiconductors, dielectrics and metals Class properties 1. Electrical properties 2. Electro-optical properties
3. Electro-acoustic properties 4. Magnetic properties
5. Thermal properties 6. Mechanical properties
Basic phenomena and processes of this class properties The movement of charge carriers and their interaction with each other and with the environment Generation and registration (detection) of optical radiation, their interaction with the environment and various fields, mutual transformation of the electrical and optical signals Generation and registration (detection) of the acoustic oscillations, the transformation of electromagnetic energy into the energy of elastic waves The emergence of different types of magnetism. The interaction of the magnetic moments of electrons with each other, with the moving electric charges and with the environment Vibrations of atoms (the motion of photons), their interaction with each other and the environment Elastic and plastic deformations
In general, the properties of materials depend on three characteristics: 1. the nature of the chemical bonding; 2. the chemical composition and the phase state; 3. the degree of perfection of the atomic structure. On the effectiveness of the influence of structural defects on the properties the properties can be divided into following groups: a) structure-insensitive properties – virtually independent or very little dependent on structural defects, determined by the nature and strength of the chemical bonding; b) the structure-sensitive properties – strongly changed under the influence of structural defects, their type and concentration. These properties are associated with the movement of particles or quasiparticles – atoms, electrons, phonons, grain boundaries, the boundaries of magnetic or electric domains and etc. § 2. Electrical properties All materials in different degrees, conducted electric current, i.e. had electrical conductivity. On this basis the materials are divided into conductors, semiconductors, dielectrics. In physics, the division into metals and non-metals is determined by the behavior of the electrical resistivity of the material: in metals is determined by the electronic structure of shells and at Т 0 К, 0, at the same time, in non-metals, i.e. in semiconductors and dielectrics at Т 0 К, . All substances due to electrical physical properties (specific resistivity ρ) can be divided into three major classes: metals: ρ = (10-6 – 10-4) Ом*см, semiconductors: ρ = (10-4 – 1010) Ом*см, dielectrics: ρ > 1010 Ом*см. These intervals are relative, because under the influence of various factors limit values ρ may overlap. The conductivity of semiconductors σ is intermediate between metals and insulators. The ability and the opportunity of the material to conduct electrical current is mainly depend on: the type of chemical bonding,
the band gap, type of free charge carriers, their concentration and mobility. The main parameters that characterize the electrical properties are: electrical conductivity γ (ohm-1 * m-1); resistivity ρ (Ohm * m); the temperature coefficient of resistivity αρ (K-1). Conductivity γ connected the current density j (A/m2) and the electric field strength E (V/m), causing the current ratio ј = γЕ
(differential form of Ohm's law). Electrical resistivity – the inversed magnitude of conductivity:
where γ – conductivity, [γ] = [Sm/m], (См –Siemens). The density of the current j is related with the charge e of current carriers, their number n and field strength by the relationship: j = еnμЕ
where μ – charge carrier mobility, numerically equal to the drift velocity of charged particles in the direction of the field strength in the 1V/cm, [E] = [1 V/cm]), [μ] – [cm2 / (V*s)]. The mobility of the charge carriers depends on the type of chemical bonding, the temperature and structural imperfections and varies for different substances within the range of from 10 to 105 [cm2 / (V*s)]. Structural sensitivity of the electrical conductivity caused by the influence of structural imperfections on the mobility of the charge carriers. In the presence of charge carriers in the material of different types (electrons, holes, or ions) the electric conductivity is determined by the expression: γ = Σ eniµi
from which follows that the contribution to the electrical charge carriers electrical conductivity of this type depends on the concentration and mobility. 12
The mobility of the charge carriers is equal to:
e l e = * * m v m
where m* – effective mass of carrier; l – length of free path; v – the thermal velocity of the movement of charge carriers; τ – mean free time or relaxation. Then
ne 2 l el m*v m*v
that is, the electrical conductivity is proportional to the concentration of charge carriers, their mobility, and the free-path length and inversely proportional to the effective mass. The free-path length of the electron is in the range 10-6 < lсм< 10-5 and the lower, the more violations of the periodic potential field of the ion core of crystal caused by the thermal vibrations of the atoms (dynamic distortion) or disordered atomic displacements caused by the dissolution of foreign atoms with atomic radius different from the matrix (static distortions). The thermal electron velocity v at nondegenerate semiconductors at room temperature equals about 10 cm/s, and in metals, where the electron gas is degenerate, the rate approximately greater to order. Hence, the average wavelength of free electrons, depending on the de Broglie relation:
in semiconductors is approximately 7*10-7 cm, and in metal to one order less 5*10-8 cm, i.e. is the same order of magnitude as the interatomic distances. It follows that the electron scattering on point defects must be strongly expressed in metals, and extended defects
(dislocations, sub-boundaries and grain boundaries) – in semiconductors. In accordance with the physical nature of the charge carriers existed two main types of electrical conductivity: electronic and ionic. Electronic electrical conductivity can be purely electronic (for metals), purely hole and mixed, when in the electrical conductivity involving both electrons and holes (semiconductors). Ionic conductivity may be cationic, anionic, and mixed. Electronic conductivity have metals, semiconductors and dielectrics. The electronic conductivity of dielectrics is observed only at very high voltages (near breakdown). Ionic conductivity have liquid electrolytes and ionic crystals (alkali-halide, and others). An essential feature of the ionic conductivity is that it is accompanied by the transfer of substance. The electrical conductivity depends on temperature, pressure, irradiation, impurities. The sharp dependence of the electrical conductivity of semiconductors from different types of affecting give them opportunity in the application as sensors. Changes of electrical conductivity of metals under all kinds of impacts, including temperature changing associated with the change in charge carrier mobility. The higher the temperature, the greater the amplitude of the thermal vibrations of atoms (ions), the more the local distortions of electric field of the ion core lattice, the stronger the scattering of charge carriers and the greater the resistivity of metal. In semiconductors increase in temperature and other effects affecting to the mobility of charge carriers as in metals, but at the same time it increases the carrier concentration, can change the bandgap and other characteristics. These changes affect to the resistivity of semiconductors more than changing the mobility of charge carriers. Therefore, in semiconductors resistivity versus temperature dependence is more complicated. Affecting the deformation to ρ (resistivity) depends on the nature of the material, the type of deformation – elastic or plastic. During plastic deformation to ρ influence the type, concentration and distribution character of structural imperfections. Changing ρ of semiconductors under the influence of elastic deformation causes 14
tensoresistive effect, which was used in the mechanical strain sensors. Plastic deformation and radiation increase the concentration of charge carriers and at the same time reduce their mobility, mostly first effect dominates, and ρ is reduced. For body with a constant cross section S, resistance R and length l, ρ is determined by:
According to the theory of electrical conductivity, γ can be expressed by the following formula:
q 2 n m
Where q and m – respectively the charge and mass of the charge carrier (electrons in conductors, electrons and holes in semiconductors, ions in dielectrics); and λ – the speed and the length of free path of the charge carrier; n – charge concentration, i.e. the number per unit volume. Changing the conductivity and consequently the resistivity in real materials related to the concentration change and length of free path of the charge carriers. Under the influence of electric field the charge carriers acquire acceleration, and their speed is proportional to the field strength:
Where u (m2/ V*s) – charge carrier mobility- the ratio of the velocity of their directed motion caused by the electric field to the field strength. It is determined by
from whence γ =qnu
The value of the electrical conductivity strongly depends on the carrier scattering by imperfections of the crystal lattice – structural defects and phonons. In the result of scattering reduced length of free path, speed and mobility of charge carriers. The electrons in an isolated atom have a strictly defined discrete values of energy. In solid in the result of atoms convergence and the strong interaction electrons and nuclei splits the energy levels of atoms and their integration into energy zones (Figure 1.2).
Conduction band Ес
E Valence band Figure 1.2. – Energy bands in solids
The energy band, where can present the charge carriers, called permitted band. Bands of energy, which may not be present carriers- band gap. During the formation of the solid from n atoms the discrete levels of the atoms are split into bands of allowed energies, which are separated by forbidden energy bands. The maximum number of electrons on discrete levels of atoms equals: levels number of electrons
In metals at the top of the energy band is always present unfilled permitted energy states. The Fermi level separates the filled part of the band from unfilled. Energy band, resulting from the splitting of the levels of valence electrons is called the valence band ( E ). After band of allowed energies – the conduction band (Ес). Between them is the band gap (Еg). When electron gets the energy exceeding the band gap, it passes from the valence band to the conduction band and participates in the electrical conductivity. According to band theory of solids metals difference from nonmetals is in the nature of the filling of the upper (last) energy bands. The most important feature of metals is that in them high energy band containing electrons (conduction band) is unoccupied levels. In dielectrics and semiconductors at low temperatures (close to 0 K) upper, entirely filled with electrons energy band (the valence band) is separated from the next – empty – band of allowed energies (the conduction band) with prohibited area Еg – bandgap, in which lacks the energy levels of electrons. In terms of the band theory of difference between semiconductors and dielectrics purely conventional: the value of Еg , which separates the valence band and the conduction band in semiconductors and dielectrics is: Еg(sc) = ≤ 2 эВ, Еg(diel.) = ≥ 2 эВ
Existed also gapless semiconductors whose Еg = 0, for example, HgTe and HgSe. Impurities and defects in semiconductors and dielectrics may give rise to levels in the bandgap. In semiconductors, the band created by the valence electrons are called valence (it is full at T = 0 K). The top of the valence band E v . Blank band at T = 0 K after bandgap called the conduction band. The bottom of the conduction band is E c (lowest energy).
According to the band model of semiconductors and dielectrics are not different. In practice, many semiconductors at low temperatures (near 0 K) behave as dielectrics, many dielectrics at high temperature is semiconductors. According to the band theory solids are divided into conductors, semiconductors and dielectrics. Conductors – materials in which the valence and conduction bands overlap or are adjacent to each other. Therefore, the electrons in the metal are free, i.e. can move from the valence band to the conduction band by applying a small electric field strength. The atoms in metals are connected with each other by metallic bonding. The valence electrons have high mobility because of the overlap E and Ес can be easily moved in the lattice of metal crystal. In metals observed electronic type of conductivity. This electrons was accelerated by the field transfer only charge. Mass transfer, such as in materials, which have ionic conductivity type does not occur. ρ Range of metallic conductors takes three orders of magnitude from 1,58*10-18 Ohm *m for silver until 1000*10-8 Ohm * m for alloys system Fe – Cr – Al. Semiconductors due to electrical properties have an intermediate place between conductors and dielectrics: their electrical resistivity is 10-6-109 ohm * m, the bandgap – from 0.05 to 2.5-3 eV. Atoms in semiconductors can be connected as a non-polar and polar covalent and ionic bonding, the type of electrical conductivity – electron-hole. As dielectrics, semiconductors have negative temperature coefficient of resistance (TCR) αρ, i.e. with rising temperature ρ of semiconductors decreases, whereas ρ of metals increases. An important feature of semiconductors is the high sensitivity of resistivity not only to heat, but also to other external influences (electromagnetic fields, radiation, etc.). This is due to the type of chemical bonding between atoms in the crystal lattice of the semiconductor, as well as presence of impurities and other defects even negligible concentrations which significantly affect to the concentration of free charge carriers and hence to the electrical properties of material. At industry used semiconductors, which have electron and hole type of electrical conductivity. 18
In dielectrics bandgap higher than 3 eV, the electrical resistivity is 109 – 1016 Ohm * m. As in semiconductors, in dielectrics can occur covalent bonding type. A feature of the electrical conductivity of solid dielectrics is in most cases it is ionic character. Since Еg >> kT, only a very small amount of electrons can break away from their atoms by the action of thermal energy, and their contribution to the conductivity is negligible. Ionic electrical conductivity may be due to movement as an impurity ions and ions of the dielectric. It should be noted that the electronic type of conductivity can be felt in the case if in the bandgap near the bottom of conduction band and top of valence band, respectively, will form a large number of donor and acceptor levels. The appearance of such levels may be due to the presence of impurities and crystal lattice defects. Electronic conductivity, due to the presence of free electrons is manifested in strong electric fields and lead to insulation breakdown. One of the major applications of metals and alloys in technique is using them as conductors. They are divided into two groups: • Metals and alloys with high conductivity • Metals and alloys with high resistance. Metals and alloys with high conductivity is used for making the conductors, wires, cables, contacts, transformer windings, in integrated circuits for creating current carrying elements and others. The high electrical conductivity have pure metals – Ag, Au, Cu, Al and their alloys, some steels, bimetals. The main requirements to them – low resistivity and low temperature coefficient of electrical resistivity. Metals and alloys with high resistance are used for the manufacturing of resistors, rheostats, electric heating devices, and others. These include copper alloys (constantan, manganin, nickeline) and alloys system of Fe – Ni – Cr, Fe – Cr – Al. Basic requirements for them: high ρ, low and low thermoelectric power in tandem with copper. Furthermore, the alloys for electric heating devices have to be fire resistant. Apart from these requirements as conductor and resistive materials must have a high mechanical strength, corrosion resistance
and workability, i.e. processability pressure, welding, soldering, and other types of processing. Changing values γ and ρ in real conductors is primarily due to the change in the length of free path λ. The electrical conductivity of metals depends on the incompleteness of the valence shells, overlap of electron shells. IB- subgroup (Ag, Cu, Au) and IIIB-subgroup (Al) elements of the periodic system have the highest electrical conductivity. This is due to the fact that the electrons easily move in the electron gas from incomplete s- shells. IA-subgroup elements, although they have the same structure of the outer s-shell exhibit lower conductivity due to the low conduction electron concentration (n), which is determined by the ratio of the crystal lattice parameters and diameter of the ion. The transition metals have higher ρ than non-transition. In transition metals occurs overlap s- shells by unfilled d- and f- shells, which are energetically located below s – shells. When an electric field is applied occur scattering of s – electrons in the d – and f – bands, reducing their concentration in the conduction band. Thus, the resistivity of pure metals are determined primarily by their nature, i.e. the concentration of conduction electrons. It does not depend on the temperature and the actual observed changes in ρ by varying the temperature associated with the change of the length of free path and the electron mobility. During passage of the electron wave through an ideal (defectfree) lattice scattering do not occur. Crystal lattice defects is a cause and, of electrons scattering, resulting in the reduction of consequently, increase ρ. Imperfections, which scattering electrons, can be divided into two groups: – energetic defects (thermal vibrations of atoms or ions of lattice), determined by the temperature component (ρТ) of material resistivity; – defects of crystal structure, determined structural or residual (ρres) component of the resistivity of the material. In this regard, the electrical resistivity of pure metal can be represented as ρ = ρт +ρres 20
The impurity and intrinsic defects that violate the periodicity of the crystal lattice are the centers of scattering of electron waves. This reduces the length of free path λ and increases resistivity. In a wide temperature range dependence of ρ from temperature is expressed as following: ρт = ρ0(1+αt+βt2+γt3+…)
In the temperature range for t> Θd (Θd-Debye temperature) ρ linearly depends on t: ρт= ρ0(1+αt)
Or during choice of absolute temperature scale ρт= ρ0αТ
where ρ0 – resistivity at temperature taken as the reference point; T – the temperature (K); α = αρ – temperature coefficient of resistivity. Debye temperature separates the "low" temperatures area, in which quantum effects occur and where it is necessary to use quantum statistics, from the area of "high" temperatures. In the differential form αр = (1/ρ0) (dρ/dT). At T=Tm resistivity increases abruptly due to sharp decrease in the concentration of conduction electrons. Some metals and alloys at temperatures close to 0 K, transfer to superconductive state i.e. their ρ sharply decreases almost to zero. In superconducting transition temperature (Тс) ρ < 10-18 Om*m. The theory of superconductivity based on the assumption that the electrons carrying the process of electrical conductivity connected Cooper pairs, the electrons in such pair have opposite directions of spins and impulses. Such binding of electrons is possible in the medium containing the positively charged ions, which weakens the field strength of the Coulomb repulsion between the electrons. The
nature of the attraction forces between electrons is determined by their interaction with phonons. Movement of electron pairs can be viewed as the motion of one electron wave, which does not scatter by lattice points, and "wraps around" them. At T=0 all conduction electrons are connected. Rising of temperature and increasing of thermal vibrations leads to the rupture of the pair, and in Тс all pairs are destroyed, superconductivity disappears and the metal goes into a normal state with finite value of the electrical conductivity. Unlike pure metals in the lattice of the alloy of main material arranged atoms of another element or formed other phases. In both cases they represent the scattering centers of electron waves. For alloys, as well as for pure metals, performed dependence: ρ = ρт +ρres. For different types of alloys the dependence of the resistivity from the concentration of components forming the alloy is different. Effect of solute on the electrical properties of alloy due to violation of the periodicity of the electric potential of main component lattice. These defects lead to scattering of electrons, decrease of the length of free path and, consequently, to increasing of ρ. The degree of change of ρ depends on the nature of the main and impurity component – their valence and atomic diameter. The greater the difference between the valences and atomic diameters, the greater the increasing in ρ. In the case of unbounded solid solutions of components A and B, if A and B – non-transition elements, ρост increases by dissolving B in A as A in B. In this change in ρ depending on the concentration of the components is characterized by symmetrical curve with maximum. The dependence of the length of free path from the concentration of components A and B in the alloy is expressed by the relation: λ = β/(сАсВ) = β/(сА(1 – сА))
where β – coefficient of proportionality, constant for this system; сА and сВ – respectively, the concentration of main and impurity component (at.%). Substituting this expression into the formula ρ = m T/ (e2nλ), we obtain 22
ρ = m TсА(1 – сА)/ (e2nβ)
By grouping the constant factors and denoting m T/(e2nβ)=D, we obtain ρ = DсА(1 – сА)
The function сА(1 – сА) – parabola with maximum at сА= ½, i.e. during equiatomic ratio of component in the alloy. Examples of such alloys are Ag – Au, Cu – Au, W- Mo. The temperature coefficient of electrical resistivity of alloys is defined as same as for pure metals with using formula αp all = (1/ ρ0all) (d ρall /dT )
In isometric conditions αp all 1/ ρ0all. If one of the components of solid solution transition metal, the concentration dependence differs from parabolic. Because of s – d or s – f – electron scattering in transition metal maximum of ρ shifts toward higher concentrations of transition metal. If the transition metal are both components, then there is not only maximum displacement, but also took place velocity fluctuation of the curve. The concentration dependence of the resistivity of eutectic alloys have linear character, as eutectic composed of phases, each of which has its own electronic structure, crystal lattice and concentration of conductive electrons. Eutectic phases can be pure metals, solid solutions or chemical compounds. In the case of changing concentration of components proportion of the eutectic phase change additive, as additive from one phase to another boundary phase and electrical resistivity of the eutectic. The electrical resistivity of eutectic two-phase described by ratio ρevt = ρ1 с1 + ρ2 с2 , where ρ1, ρ2, с1, с2 – respectively, the electrical resistivity and concentration of the first and second phases. In practice, there is disruption of the linearity of concentration dependence of ρ eutectics due to the presence of impurities, grain boundaries and other defects. The temperature coefficient of eutectic
resistivity as αр, of solid solutions, varies inversely with the concentration changes of ρ. In contrast to solid solutions and eutectic chemical compound it is a brand new substance is fundamentally different in structure and properties of its constituent components (another type of crystal lattice, electronic structure, the concentration of charge carriers, sometimes another type of chemical bonding and electrical conductivity). Metal films produced by vacuum methods (e.g., thermal evaporation, ion-plasma sputtering) used in microelectronics as interconnections, contact area, resistive and the magnetic elements, capacitor coatings. The electrical properties of thin films are substantially different from those of the starting materials in bulk state. This is due to: – structure of the films. At condensation of sprayed metal on the surface of the film structure can be changed from amorphous to crystalline; – size effects. In the film prevail surface processes over bulky processes, especially if the film thickness (h) is comparable with the length of free path (λ) of majority charge carriers, which influence on the properties including electrical properties. The resistivity ρ of the films is always above ρm due to the high concentration of defects. The increase in ρ also contributes and size effect, i.e, decreasing the length of free path of electrons due to the scattering from the film surface. The electrical properties of semiconductors The most important elementary semiconductors, such as silicon and germanium, have the structure of the diamond, and many semiconductor crystals such as А2В6 or А3В5 (e.g., CdS, SdTe, GaAs, GaP, InSb, InP, AlP, AlSb, ZnS, etc.) have the structure of sphalerite type. The main type of chemical bonding in semiconductors – is covalent bonding. Typically, covalent bonding (covalent non-polar) occurs when the socialization of valence electrons of neighboring atoms and elements observed in IVB-subgroup of the periodic system (Si, Ge), where each atom has four valence electrons. To form the connection each atom can take four electrons from each of four neighboring atoms and can also give them the same number of electrons, while remaining electrically neutral. Thus, occur exchange 24
of electrons between atoms with forming stable eight electron valence shell of each of them. Also the class of diamond-like compounds include А3В5 compound semiconductors, which form by IIIB- (B, Al, Ga, In) and VB- (N, P, As, Sb) subgroups elements of the periodic system and counterpart electronic analogues of Si and Ge. The atoms of III group elements have three valence electrons, while V group elements have five. Thus, to one atom in these compounds have an average of four valence electrons. Since the electron cloud in this regard, strapped to more electronegative atom B, it is not completely covalent and partially ionic (such bonding called covalent polar). Where A is charged positively and B negatively. Even more ionic component of chemical bonding expressed in А2В6 compounds (ZnTe, ZnSe, CdTe, CdS, etc.). Finally, there are semiconductors with ionic bonding – are lead chalcogenides (PbS, PbSe, PbTe). Qualitative characteristic of chemical bonding compound is its average atomic number Zav. For simple compounds А3В5 and А2В6 Zav =(ZA+ZB)/2
Within a class of compounds with increasing Zav increases tendency of transistion from covalent to ionic bonding. This leads to the reduction in bonding strength; decreases also bandgap, melting point, resistivity. The charge carriers. Intrinsic carrier. As a result of the electron exchange between atoms in the formation of covalent bonding the electrical conductivity does not occur, as the electron density distribution is fixed (two electrons for bonding between each pair of neighboring atoms). Under the influence of external effects (e.g., heating, irradiation) can occur rupture of one of the bondings, and electron leaves it, becoming free in crystal. He moves randomly through the crystal in the absence of an electric field. The absence of electron from one of the atom bondings is called the hole, and means that there is positive charge, which equal in value to the charge of past electron. The hole, as well as the electron moves randomly
through the crystal, since the electron of neighboring bonding may take the place of the departed electron. Semiconductor, which electrical conductivity caused by the movement of their own charge carriers, called intrinsic. Formation of electron-hole pair is called the generation of charge carriers. This generation is possible in the case if electron energy exceeds Еg the band gap; in this case, the electron passes from the valence band to the conduction band (i.e. leaves the potential well of their intrinsic atom and detached from it); in the valence band formed hole. Thus, the band gap is the minimum energy that must be expended in order to snatch an electron from the covalent bonding. Note that if the electron energy does not exceed Еg, the formation of an electrically neutral bounding pairs of electron – hole, called an exciton. The excitons can play a significant role, for example, in the formation of color centers in alkali halide crystals. In ideal crystal the concentration of electrons and holes are equal and grow with the increasing the number of violations of covalent bondings. At the same time due to the presence of impurities and structural imperfections in the band gap can be present levels allowed for electron energies. These levels can be occupied by electrons or remain vacant. If the electron passes from the valence band to the allowed vacant level in bandgap or from occupied level to the conduction band, then occur generation of extrinsic charge carriers. Extrinsic carriers. Sources of extrinsic charge carriers are electrically active impurity atoms. They may be atoms of elements constituting with semiconductor substitutional or implantation solid solutions and have a valence different from the valence basic atoms. Impurity atoms are divided into: • donors, which gives excess electrons, because they have a high valence; • acceptors, exciting valence electrons of the basic substance, as they have lower valence; Donors created in semiconductor electronic conductivity (n-type conductivity), acceptors created – hole conductivity (p-type conductivity). Appropriate semiconductors called electronic (n-type) and hole (p-type). For elementary semiconductors (Si, Ge) donor is V group impurity atoms (P, As, Sb), while III group (B, Al, Ga, In) is acceptor. Donor and acceptor impurities called dopants. Doping- is 26
the creation of semiconductor with predetermined conductivity type by introducing into its composition dopants. Arsenic atom has five valence electrons, atom of silicon – four, i.e. one electron of arsenic is not participate in the formation of covalent bonding. It is associated with its atomic strength of Coulomb interaction, which energy is comparable at room temperature with the energy of thermal motion (kT ~ 0,03eV). Therefore, the fifth electron of arsenic is easily detached from their atoms and become free, while the atom – a positively charged ion. Creating of semiconductor with certain type of conductivity is very important, since the principle of many semiconductor devices action based on the impurity conductivity. As for the ionization of both donor and acceptor impurities require energy, less than needed to break covalent bonding, that is, to form their intrinsic carriers (Еext 1,0 µm). Various characteristics of optical irradiation – the intensity, frequency of phase, polarization, and others can change the time according to given law. Light modulation can be carried out in various ways, e.g., by using various types of mechanical breakers. The most interesting and gives possibility of using physical effects – electrooptical, magneto-optical, elasto-optical accompanying the propagation of light streams in different conditions and environments. § 4. Acoustic properties Acoustic properties are properties associated with the generation, detection, and various kinds of interaction with the medium of elastic vibrations and waves of very low frequency (from 0 Hz) to extremely high (1011 – 1012 Hz). The frequency range from 16 Hz to 20 kHz detected by the human ear, the range below 16 Hz is infrasound, above 20 kHz – ultrasound, high frequency range 1012 – 1013 Hz – hypersonic. A special case of acoustic waves are surface acoustic wave (SAW). These waves propagate along the free surface of solid or along the borders of solid with other media. At distance from the border, these waves are damped. SAW can be in two types: 1) with vertical polarization, when the elastic vibrations of the medium particles under the influence of SAW occur in the vertical border of plane; 2) with horizontal polarization when these fluctuations are parallel to boundary and perpendicular to direction of the wave propagation. Elastic acoustic waves are generated by any phenomena caused by local changes in pressure or mechanical stress. Different sources generate acoustic waves of different frequencies. Acoustic wave propagation is characterized by the speed of sound сs. The speed of sound is very small compared with the speed of optical irradiation (light). It depends on the aggregation state and nature of the material: сs. in gases less than in liquids, and in liquids
less than in solids. In Table 1.4. given the values of sound speed for some substances. In isotropic solids сs depends on the elastic moduli, in anisotropic solids speed of sound is anisotropic. In piezoelectric and ferroelectrics сs depends not only on the elastic moduli, but also on the piezoelectric coefficients and the strength of electric field, while in ferromagnetics – from the strength of magnetic field. Table 1.4. Speed of sound in some substances № 1 2 3 4 5 6 7 8 9
substance Air Hydrogen Water Mercury Gold Glasses Iron Fused quartz Aluminium alloys
speed of sound сs, m/s 331 1284 1490 1453 3200 3760 – 4800 5900 5970 6000
Measurement of сs is used to determine the elastic moduli of solids, the Debye temperature for the investigation of the band structure of semiconductors, the definition of the Fermi level in metals and others. In the propagation of sound wave occur absorption of sound, which much weaker than the absorption of the optical irradiation. Absorption is associated with the transition of the sound wave energy into other forms of energy, mainly in the heat. The consequence of this absorption is sound attenuation, i.e. reduction of its intensity and amplitude. In the propagation of acoustic waves of high intensity (amplitude) as the passage of the optical radiation of high intensity, take place phenomenon of nonlinearity. This diffraction of waves and scattering of sound become dependent not only on the frequency and speed of sound wave, in linear acoustics, but also to the amplitude of wave, sinusoidal wave is distorted, occur sound pressure of irradiation, etc. The effect of non-linearity due to the fact that the propagation of acoustic waves of high intensity changes the properties of the 40
medium itself, which affects both the propagation of the waves and other disturbances. Interaction of acoustic waves with electrons have particular importance in electronics and called acoustic-electronic interaction (AEI), while interaction with electronic waves called acousticoptical interaction (AOI). AEI manifests itself in the ultrasonic and hypersonic vibrations with frequency 107 – 1013 Hz, when under the influence of propagating acoustic wave occur elastic deformation of the crystal lattice and changing its intracrystalline field. The energy and momentum of ultrasonic and hypersonic waves transmitted by conduction electrons (particular case of the electron-phonon interaction). The transfer of energy results to additional electronic absorption of sound and heating of the electron gas, while transfer of momentum
h – to the emergence of current or e.m.f. in metal or c
in semiconductor (acoustic-electric effect) in the direction of sound propagation (entrainment effect). In addition to changes in the electrical conductivity, AEI changes the heat and thermal conductivity. AEI mechanism is different for crystals of different nature. In ionic crystals and metals have the ionic interaction – acoustic wave displaces the ions from their equilibrium position, occur ionic current and field, which acting to conduction electrons. In number of semiconductors (Ge. Si) and semimetals (Bi, Sb, As) realized the potential – deformation interaction – under interaction of ultrasonic wave changes the bandgap, occur regions with lower and higher charge density acting on the conduction electrons. In piezoelectric semiconductor of АIIBVI (CdS, CdSe, ZnS, ZnO), III V A B (InSb, GaAs) and in others manifest piezoelectric interaction – the deformation of these crystals is accompanied by occurring of electric field and vice versa. From the mechanism of AEI depends magnitude of the electronic absorption of ultrasonic waves. It is maximal in piezoelectrics. In metals and in conventional semiconductors electron absorption becomes noticeable only at low (helium) temperatures.
The transfer of ultrasonic wave impulse by conduction electrons leads to acoustic- electric current. If to the crystal applied also constant external electric field E, which creates electron drift in the direction of the ultrasonic wave, then AEI depends essentially on the drift velocity vdr and propagation velocity of sound сs. When vdr < сs ultrasonic wave is absorbed by the electron gas at vdr>сs electrons give their kinetic energy to ultrasonic wave, occur strengthening (increasing of amplitude). This increase has practical interest for the surface acoustic waves. AEI leads to number of non-linear acoustic effects, is particularly noticeable in piezoelectric materials used in acoustic electronics, in memory elements. Most of the acoustic-optic device works on the phenomenon of light diffraction by ultrasonic waves. Elastic deformation in the sound wave leads to periodic change in the refractive index n of the medium. As a result, in the medium occur structure similar to diffraction lattice having period equal to the wavelength of sound λs. If at such medium distribute light beam, the medium will have diffraction light beams. Their characteristics – direction in space, polarization, intensity – depends on the sound field parameters (γ, I) and the angle θ, at which the light falls on the acoustic beam. The frequency of the diffracted light is different from the frequency of the incident light on magnitude of the sound frequency. At the exit of the acoustic beam light wave is modulated in phase and deviate from direction. Interaction of sound waves in solids and liquids with optical irradiation is effectively used in electronics, laser technology, optics to control the amplitude, polarization, spectral composition and direction of propagation of the optical beam. With the help of the diffraction of light by ultrasonic waves are determined by the characteristics of the sound field, absorption, and the speed of sound, elastic modulus of elastic-optical and magneticoptical materials, created apparatus for receiving signals in ultrasonic delay lines. In interaction, which propagate in the crystal of ultrasonic and hypersonic waves with frequency from 10 mHz to 1.5 GHz with each other and with electrons, as well as application of surface 42
acoustoelectronic devices based on acoustic waves for the conversion and processing of electrical signals. § 5. Magnetic properties The substances have magnetic properties due to the magnetic moment occur because of the motion of electrons (the magnetic moments of the atomic nuclei approximately thousand times smaller than the magnetic moments of electron). There are two main types of electrons motion, leading to the appearance of magnetic moments: orbital (orbit around the nucleus) and spin (on its axis). Accordingly, there are the orbital and spin magnetic moments. Spin magnetic moment equal to one Bohr magneton, J/T: Мm sp =
h = 9,273 * 10-24 2m 2
where e, m – charge and mass of the electron. In addition to these two main types of electrons motion, there is another, which is manifested in the application of an external magnetic field. In this case, an electron moving in closed orbit, changes its trajectory: instead linear it becomes spiral. By its nature existed following types of magnetism: diamagnetism, paramagnetism, ferromagnetism, antiferromagnetism and ferrimagnetism. In Figure 1.5. shown the orientation of the magnetic moments.
Figure 1.5. – Orientation of the magnetic moments of neighboring atoms at 0K in materials with different magnetic nature: 1 – paramagnetic; 2 – ferromagnet; 3 – antiferromagnetic; 4 – ferrimagnet
Let’s talk about the main magnetic characteristics. The magnetic moment of body М equal to the product of the magnetization J on the body volume V: М=JV (1.40) The magnetization of the material – its ability to change its magnetic moment under external magnetic field strength H is characterized by magnetic susceptibility æ: J=æН
The resultant magnetic field in the material known as magnetic induction B. The value of B is associated with the strength of external magnetic field H and magnetization of the substance J by relation: В = Н + 4π J
The ability of substance to change its induction В in under the influence of the external field H is characterized by permeability μ: В = μН
Dependence of J, and B, and therefore, μ from H are nonlinear. The limit value of μ when strength H tends to zero, called the initial magnetic permeability μi. Magnetic permeability is related with the magnetic susceptibility by ratio: Μ = 4π æ + 1
The physical nature of diamagnetism is associated with the rotation of spiral electron by closed orbits induced by the external field and gives rise to undamped eddy microcurrents. Internal magnetization arises in the body under the influence of an external magnetic field and directed toward the field, so the diamagnetic susceptibility æmD has negative value. The main contribution to diamagnetism of atom make outer electrons. Diamagnetism enjoyed all substances without exception. 44
But the prevailing type of magnetism occur only in substances with filled electron shells: inert gases, Na+, Cl-type ions, semiconductors (germanium, silicon, selenium, etc.). If substances along with diamagnetism have other kinds of magnetism, then role of the latter covers the role of diamagnetism. The diamagnetic susceptibility of the solids are in order of 10-5 – 10-6 Gs/E (Gauss to oersted). Under paramagnetism understands the property of body to magnetize in external field H in the direction of the field. Consequently, the paramagnetic susceptibility has positive value. Therefore paramagnetic bodies are attracted to the poles of the magnet, while diamagnetic and repelled. The total magnetization of paramagnetics equal to the sum of external and internal fields. The main feature of the paramagnetic bodies is that they have their own magnetic moments of the atoms (orbital and spin), but due to the interatomic interaction magnetic orbital angular moments of two paired electrons canceled each other. In the result all filled electron shells and orbitals have zero orbital magnetic moment, and did not contribute to the paramagnetic properties. Paramagnetism is found only on the unpaired valence electrons – the conduction electrons. Spin moments do not experience such interaction of the crystal field, and therefore their contribution to the magnetic moment of atoms in solids is significant. In the absence of external field, the magnetic moments of atoms due to thermal motion oriented randomly, causing the magnetization of paramagnetics under these conditions is equal to zero. This is difference from ferromagnetics. When an external magnetic field H applied moments of atoms predominantly oriented along the field. With increasing H magnetization of paramagnetic increases by law J=æmpН, where æmp– magnetic susceptibility of 1 cm3 substance (for paramagnetics æ is equal to 107 – 10-4). If the field H is very large, all magnetic moments are oriented along the field, occur magnetic saturation. With increasing temperature at constant H increases disorienting effect of thermal motion.
The substances in which no conductive electrons, magnetic moments of electron shells of atoms compensated and magnetic moment has only nucleus. The paramagnetism of such substances is very small (10-9 – 10-12) and can be observed only at very low temperatures (T = 0.1 K). Nuclear paramagnetism in the absence of strong interaction between the spins of nuclei and electron shells of atoms characterized by the value æmn=
NM mn 3kT
where Mmn – magnetic moment of nucleus equals approximately to 0,001 of the magnetic moment of electron, from which æmn≈10-6 æme. Research of paramagnetic properties with using electron paramagnetic resonance (EPR) and nuclear magnetic resonance (NMR) allows to determine the magnetic moments of the individual atoms, ions, molecules, nuclei, to study the structure of individual molecules and complexes, to carry out thin structural analysis of materials. For this purpose used the sharp demagnetized paramagnetics in thermal insulation conditions (adiabatically), in which the spins acquire random orientation, accompanied by decreasing in temperature (magnetic cooling). Ferromagnetism as paramagnetism associated with the spin magnetic moments of electrons. But in contrast to the paramagnetics in ferromagnetics have separate microregions (domains), which below of certain temperature (Curie temperature Тс) spin moments of all atoms have the same orientation in the absence of external magnetic field. The domain is the microregion about micrometer, spontaneously magnetized to saturation at temperature below Tc. In the absence of external field the magnetization vectors of different domains are oriented randomly and canceled out. When external magnetic field applied the magnetization vectors of all domains gradually reoriented along the field. Upon completion of this process (in fields N≈8 kA/m) achieved limit value of magnetization JS and induction Вm. Value of JS is maximal at T = 0K. 46
With increasing temperature JS decreases and at T= Tc become equal to zero, the ferromagnetic transite to the paramagnetic state. The emergence of domains due to the fact that the exchange interaction decreased the energy of neighboring atoms, but at the same time increased the amount of the total magnetic moment of ferromagnetic volume and magnetic- static energy (magnetic field, distribution to environment). Minimizing of total magnetic energy is achieved by splitting into domains. For the spontaneous magnetization must honored the following two conditions: 1) the presence of uncompensated spins; 2) the ratio of the interatomic distance of neighboring atoms а to the diameter of electron subshell with uncompensated spins d must
a =2÷5. d a 5 exchange interaction within domain is reduced, ordering d
in spin orientation is absent. State of body will be paramagnetic. In addition to the exchange interaction between the spins of neighboring atoms in the crystal take place interaction between the spins and the lattice atoms, because of which the total magnetic moment arranged along certain preferred crystallographic directions, called as the axes of easy magnetization: for bcc, < 111> for the fcc and for г.к. The energy of the magnetic moments is minimal when they are oriented in the direction of easy magnetization. The work done by external magnetic field to rotate the magnetization vector Ji from the light direction to hard direction of magnetization, called the energy of magnetic anisotropy Ean. Domains with different orientation are separated from each other by transition region, in which the orientation of spins smoothly transite from one domain to another orientation. These transitional areas are
very similar to the grain boundaries in polycrystalls. They have high energy, and tends to reduce the overall system energy to migrate towards the domain of higher energy, thereby reducing its volume. The thickness of the border is usually smaller to one order than the size of domain. In thin magnetic films can be arrange orderly movement of domains and even individual fragments of the domain boundary, creating appropriate controlling magnetic field. This principle is implemented by storage devices with cylindrical magnetic domains (CMD memory), and number of magnetic-optical devices for controlling the light beam. Among the most important characteristics of magnetic materials that define the field of application limiting form of the hysteresis loop. Ferromagnetics with narrow hysteresis loop and low coercitive force (Hc 4.0 kA/m) – magnetic solid. If necessary, to maximally reduce the magnetic losses Hc can not exceed few tens of amperes per meter. The magnetic interaction of electrons is also changing the interatomic distances and therefore the size and shape of the body – this phenomenon is called magnetostriction. This phenomenon is associated with change in the magnetic and exchange forces and difficult depending on the field strength, the electronic structure – valence electron, crystallographic direction, impurities and others. In ferromagnetics magnetostriction reaches significant values. l Elongation in them may have value 10 5 10 3. The largest l magnetostriction possess some rare earth metals. For example, in l dysprosium 1.2 10 3 , which is 30 times larger than in nickel. l Magnetostriction of different materials can vary not only the absolute value but also sign of size changes. Magnetostriction is widely used in ultrasonic generators, delay lines, and others. Do not confuse magnetostriction with another phenomena- changing the magnetization of ferromagnetic body during deformation (magneticelastic effect). Simultaneous exposure to deformation and magnetization can change the value of Hc, to facilitate or impede the magnetization, to change the shape of hysteresis loop. 48
In some solids exchange interaction of neighboring atom’s electrons occur at certain temperature (below the Nel temperature TN) antiparallel spin ordering, antiferromagnetism, in contrast to what occurs in ferromagnetics. At temperatures above ТN substance is paramagnetic. Examples of antiferromagnetics is manganese oxide MnO. Do not fully compensated antiferromagnetic ordering of the spin magnetic moments called ferrimagnetism. The most important ferrimagnetism are the ferrites- ionic compounds with general formula MFe2O4 (or MO Fe2O3), where M – metal. The magnetic field strength H (A/m) proportional to the current flowing through the conductor. It can be calculated for infinitely long linear conductor by the formula Н=I/2πr and for toroid and for infinitely long solenoid H=nI, where r – distance from the conductor to the point where the field is measured, n-number of turns per unit length of the solenoid, I-current flowing through the conductor (A). The magnetic moment M (А m2). Any substance placed in magnetic field of strength H, magnetized and will have magnetic moment. Its value can be directly measure by magnetometer. Magnetic moment also has circular current: M= IS, where the S-the area of current. The magnetization J (A/m) – the magnetic moment per unit volume J=M/V. The magnetization is related to the magnetic field strength by ratio J = χmH, where χm – magnetic susceptibility – quantity characterizing the ability of substance to change the magnetic moment under external magnetic field. For vacuum χm = 0. The magnetic induction B (T) – the magnetic flux passing through unit area perpendicular to the force lines of uniform field, w2hich determined by the formula В=Ф/S=QR/S, where Ф –flux, Q –is the number of electricity induced in circuit with resistance R, with 1T = 1kl ohm / m2. Magnetization in external magnetic field body creates its own field. Relative magnetic permeability and magnetic susceptibility are related by μ = 1 +χm.
The classification of materials for their magnetic properties According to the magnetic properties materials are divided into groups: 1) diamagnetic; 2) paramagnetic; 3) ferromagnetic; 4) antiferromagnetic; 5) ferrimagnetic. The diamagnetic materials are magnetized in direction opposite to the external magnetic field. Magnetic susceptibility χm >0 and up to several thousand) similar as paramagnetics have uncompensated spin moments (Fig. 1.4 (2)). In ferromagnetics, existed areas of spontaneous (inadvertent) magnetization, called domains. Each domain is magnetized to saturation, i.e., inside the magnetic moments of neighboring atoms are arranged in parallel through the parallel electron spins of unfilled shells. This is due to the exchange interaction of the electrons. The exchange interaction is implemented in the crystal lattice under overlap of the electron shells of neighboring atoms. The electron of one atom is partly owned by another. As result, the energy system will be different in the case of parallel and antiparallel orientation of the spins. The energy of the exchange interaction is given by Eexch=– 2As1s2cos , where s1, s2 – the resulting spins of the atoms, – the angle between the vectors of this spins, А– constant of exchange interaction (is the energy difference between two electrons with parallel and antiparallel spin orientation). If A> 0, Еexch is minimum at =0, in the case of parallel orientation of the spins. In this case, the material is ferromagnetic. 50
If A 0 K in the semiconductor, electrons emerge in the conduction band and holes in the valence band. The carrier concentration in bands, especially at low temperatures is small. In intrinsic semiconductor, the Fermi level can be regarded generally as the level, which is excitation of electrons and holes when casting them as result of temperature fluctuations in the conduction band and valence band. The position of the Fermi level in intrinsic semiconductor differs sharply from the level position (surface) of Fermi in the metal; in addition, the concept level (surface) of Fermi for metal and semiconductor includes different physical content. 90
Elements of IV B subgroup – carbon (diamond), silicon, germanium, - tin. Valence shells of free atoms of these elements consist of (ns)2(np)2 –electrons. sp3 bonding- hybrid tetrahedral angle with 109028'. Hybrid binder of orbitals formed by the interaction of the valence electrons, the wave functions of which are: Ψ3s– Ψ3p for silicon, Ψ4s– Ψ4p for germanium and Ψ5s– Ψ5p for – tin. All these functions are similar to Ψ2s– Ψ2p for diamond. The above mentioned elements of IVB subgroups have diamondtype lattice, which can be represented as formed by two FCC lattice inserted into one another and mutually displaced along the space diagonal to one-quarter of its length. To one cell of lattice have eight atoms with coordinates (000, 0
1 1 1 1 1 1 1 1 1 1 3 3 3 1 3 3 3 1 , ; 0 ; 0; ; ; ; ). The 2 2 2 2 2 2 4 4 4 4 4 4 4 4 4 4 4 4
arrangement of atoms such that each of them is surrounded by four equidistant neighboring atoms (the coordination number is 4), forming tetrahedral group. Covalent bondings are directed along the and continuous permeate "bonding" of entire crystal. Elements of diamond symmetry – 3L4. 4L3. 6L2. 9p, C. The
1 1 7
coordinates of the center of symmetry , , . 8 8 8 Compact factor of lattice-type diamond is 0.34, that is, half less than for BCC. Internode are tetrahedral and octahedral voids. The radius of the sphere inscribed in the tetrahedral and octahedral interstices, close to the radius of atom. Such looseness of lattice due to the bonding direction, which significantly affects to the features of point defects formation (lighter than in metals forming Frenkel defects), the solubility and diffusion of impurities in the diamond-like semiconductors. The energy spectra of valence electrons in crystals of IVB subgroups elements is different, and the structure of valence bands of these substances are less dependent on the individual characteristics of the chemical bonding than structure of the conduction bands. Consider the results of study of the silicon and germanium band structure. Since the translational symmetry of diamond lattice is the
same as for FCC lattice, the first Brillouin zone of substances with the diamond structure is cuboctahedron. The shape of Brillouin zones depends only on the lattice structure. Therefore Brillouin zone substances having different chemical bondings, but which crystallize in similar structures are similar. In the formation of crystals of germanium and silicon valence sand p- levels of free atoms are split into two groups, creating two non-overlapping zones of allowed energies – the valence band and the conduction band. Extreme points of the conduction band of germanium and silicon lie on the axis of symmetry of the first Brillouin zone (the axis of symmetry of the first Brillouin zone in kspace: the direction of and , total 14 axes of symmetry: 8 and 6 ). The structure of the conduction band of silicon and germanium is different. In silicon minimums of conduction band are associated with at least minimum of one р- bands, which located in near the X points. Because of the symmetry conduction band has such six minimums (valleys). The surfaces equal to electron energy (isoenergetic surfaces) are spheroids. In the conduction band of silicon s-band lies above p – band. In the conduction band of germanium mutual arrangement of sand p-bands is different: minimums of the conduction associated with minimums of s-bands and located in at the boundaries of the Brillouin zone; totally existed such eight minimums (valleys). Isoenergetic surfaces are semi-ellipsoids of rotation. Thus, silicon and germanium are multivalley semiconductors with an energy equivalent to valleys. The dependence of electron energy on the quasimomentum near the minimums in silicon and germanium described by parabolic anisotropic dispersion laws. At thermodynamic equilibrium the conduction electrons are evenly distributed between the valleys. Due to the fact that the ellipsoidal surfaces of equal energy in conduction bands of silicon and germanium are arranged symmetrically, some electrical properties (electron mobility etc.) are isotropic. Equivalence of "valleys" in the conduction bands in germanium and silicon may be broken during the deformation (for example, uniaxial compression) of the crystal, in this case the energy of electrons in one valley may increased, while in others – 92
decrease. This in turn can lead to redistribution of the electrons between the valleys and, consequently, to change the resulting properties (for example, changes in electron mobility and hence change in electrical conductivity). The valence bands of silicon and germanium are similar: they consist of three energy bands. Two of these bands meet in the center of the Brillouin zone, the third cleaved from the first two by small band of the spin-orbit interaction. Thus, the maximum of the top of valence band in silicon and germanium located in the center of the Brillouin zone. The density of states in the valence band of germanium and silicon is four electrons per atom. Laws of holes dispersion in the valence band are not parabolically isotropic and distinguished from dispersion law of electrons in the conduction band. It should be emphasized that in the case of non-parabolic isotropic dispersion laws of electrons and holes (i.e. those areas dispersion characterized germanium and silicon) effective mass of the states density of electrons and holes (mnd and mpd) and effective masses of electrons and holes that define the mobility (mn and mp ) did not equal. The resulting value of the effective mass in the case of several types carriers, determining the carrier mobility in electric field called as effective mass of conductivity. According to the band structure diamond is similar to silicon. Common in the band structure of diamond, silicon and germanium crystals is the fact that at minimum of conduction band bottom does not coincide with the maximum of valence band, and therefore in these substances can only be indirect transitions. Tin has polymorphic transformation. Low-temperature semiconductor modification (α-Sn) with diamond structure transform to high temperature metal modification (β-Sn) with the structure of tetragonal lattice. Said polymorphic transformation due to the rearrangement of covalent tetrahedral bondings to metallic. Changing of bonding type in the transition α-Sn β-Sn is the reason that it is accompanied by very sharp decrease in volume (more than 20%). This polymorphic transformation demonstrates common situation that number of substances and compounds may be either in semiconductor or in metallic state, depending on temperature and other parameters related to external influences. Therefore, it would
be better to talk about the metallic and semiconducting (insulating) state of matter. The band structure of substances regularly varies depending on their position in the periodic table of elements. In Table 2.4. shown data of some properties of these elements. With increasing atomic number bondings regularly attenuated, reduced bandgap and increasing the proportion of metal component bonding. In lead following after tin chemical bonding loses direction and becomes metallic. Table 2.4. Some properties of elementary semiconductors arranged in IVB subgroup Substance
Number in periodic system
Еg, eV, at temperature, К 0 300
е , at 293 К, sm2/(V*s)
~ 1800 ~ 1550
Germanium α- tin
~ 4400 ~ 30000
* – at pressure 11*109 Pa ** – contain the transition temperature of tin from the semiconductor state to the metallic state (α β)
Another modification of carbon – graphite differs from diamond by the character of structure and significant conductivity. Graphite has layer structure; each atom in layer is covalently linked with three adjacent atoms of the same layer. One of four electrons for each atom is delocalized. These delocalized electrons cause the metallic nature of graphite conductivity. Layers linked between each other by van-der-waals forces (source of bonding type of Van-der-Waals force is polarizing effect caused by the influence of force fields moving valence electrons of another atom (molecules) in the force fields of moving valence electrons of other atom (molecules)), sharply decreases with distance. Thus, graphite is an example of complex substance with mixed bondings. Silicon and germanium was prepared, and used not only in crystalline but also in amorphous state. Silicon and germanium are 94
the main materials of semiconductor electronics and microelectronics. On the basis of these materials, especially silicon, produce the main classes of electronic semiconductor devices: diodes, transistors, photodetectors, solar energy photoconverters (solar cells) as well as integrated circuits – the basis of microelectronic and microprocessor devices. However, the "gap" of direct optical transitions in germanium and silicon eliminates the possibility of manufacturing of optical quantum generators on their basis. Silicon and germanium is produced in the form of single crystals, films and layered structures with wide nomenclature of the properties, and the production of semiconductor silicon is continuously growing. Silicon (purified significantly worse than semiconductor devices) are also widely used as alloying element in steel, especially in electrotechnical (transformer). VB subgroup elements – phosphorus, arsenic, antimony and bismuth. In V group elements are implemented chemical bondings through the formation of р3 –orbital, which, in accordance with rule of Hume-Rothery (2.3) lead to structures with coordination number ZK=3, belonging to rhombohedral syngony. Crystal with ZK=3 in particular, consisting of two-layer plates. Each atom has three nearest neighbors in adjacent layer of the same plates, with which it is linked by covalent bondings. Adjacent plates are interconnected by weak Van-der-Waals forces. Due to the fact that covalent bondings do not penetrate the entire crystal, elements of VB subgroup are more plastic than the elements of IVB subgroup. The relationship between the position in the periodic table and properties of VB subgroup elements illustrates Table 2.5. Regularities in the bandgap change are similar to above described IVB subgroup elements. In addition, it is clear that р3 bondings much weaker than sp3 bondings. VB subgroup elements are widely used in semiconductor electronics, on the other hand, as donor impurity in the elemental semiconductors like germanium and silicon, and the other – as major component of АIIIBV semiconductor compounds and several others. VI В subgroup elements – sulfur, tellurium, selenium. Chemical bonds are realized through the formation of р2 orbitals, ZK=2. Crystals of these elements consist of spiral chains or rings, in which
each atom has covalent bonding with atoms of the same chain. Between each other chain linked by Van-der-Waals forces. Links in these crystals is even weaker than in the VB subgroup. The correlation between the value of Eg and the serial number is the same as in VB subgroup (see. Table. 2.5). Table 2.5. Some properties of elementary semiconductors arranged in VВ and IVВ subgroups element
Phosphorus Arsenic Antimony Bismuth *1
15 33 51 83
Sulfur 16 Selenium 34 Tellurium 52 *1 bismuth – semimetal
shortest Т m, К interatomic distance, nm VВ subgroup 0,34 – 0,25 1090*2 0,29 903 0,31 544 IVВ subgroup – 392 0,23 494 0,29 723*3
Eg, eV, at 300 К
1,5 1,2 0,11 0 2,4 1,6 0,3
at pressure ~ 3,6*106 Pa *3 for gray crystalline tellurium
VI В subgroup elements includes as main components АIIBVI, A2V B3VI , AVI B VI and etc. numerous semiconductor compounds. In addition, they are used as donor impurities in АIIIBV compounds. VIIВ subgroup elements. Among the elements of this subgroup semiconductor is only iodine. In the solid state it has semiconductor properties, it realized p- bonding. Iodine crystals are composed of diatomic molecules bound by Van-der-Waals forces. Weak links explain the volatility of iodine. Iodine is used as donor impurity doping in semiconductor compounds, and included as component in the compounds of АIBVII type. Thus, in substances of VВ, VIВ и VIIВ subgroups bondings are pronounced heterodesmical character. Atoms in some directions or planes are linked by strong covalent, while others – weak van-derwaals chemical bonding. This greatly affects to the behavior of these substances. Since the strength of the van-der-waals bondings weaker 96
by 1-2 orders of covalent bonding strength (0.02 – 0.2 eV and 2 – 3 eV, respectively), the first destroyed by heating the van-der-waals bondings (the so-called process of sublimation) and at higher temperatures – the covalent bonding (dissociation). Solid during sublimation decomposed into atomic groups, molecules, upon dissociation – into atoms. Ease of sublimation processes explains high volatility of most substances of V – VI groups. This circumstance makes it difficult to obtain semiconductor compounds formed with the participation of these substances (АIIIBV, АIIBVI class compounds and etc.) of strictly specified composition.
PHASE EQUILIBRIUM IN SEMICONDUCTOR, DIELECTRIC AND METAL SYSTEMS
§ 1. Main aspects of the thermodynamics of phase equilibrium Real materials are compositions formed by several chemical elements. Semiconductor compound composed of two or more elements. Semiconductor thermoelectric materials include 4-5 (or more) elements, dielectric phase – 4-8 elements, etc. Modern metal alloys are often more complex compositions. Even very pure crystals of germanium and silicon always contain background impurities. Interaction of chemical elements forming this alloy can be very difficult. The result of interaction depends on the concentration of the elements, their nature and also external parameters of temperature and pressure. In the result of various elements interaction emerge chemical compounds and solutions, aggregate states, physical and chemical properties of which depend from composition, pressure and temperature. Before considering ways to describe the results of chemical elements interaction, we introduce the necessary thermodynamic concepts. Material system – part of the space allocated for various signs and filled with substance or substances. The space, which is separated from the material system, called as external environment to the system. The thermodynamic system – is material system, between the parts which can exchange energy. Physico-chemical system – the thermodynamic system, between the individual parts which can be exchanged substance. For example: 1) The system of two bodies – vials and placed in it melt. The melt do not wet the wall of ampoule and between the melt and 98
ampoule no chemical interaction. The combination of these bodies (ampoule with substance) are 1 thermodynamic and 2 physicalchemical systems (ampoule and melt). 2) The set of two bodies: crystal in contact with the melt of the same substance – one physical and chemical system. One substance in the solid and liquid phases (during crystal growth). Closed system – a system that can not exchange matter with the external environment. Adiabatic system – a system that can not exchange energy with the external environment. Insulated (closed) system – a system that can not exchange neither substance nor energy with the environment. Open system – a system that can exchange either energy or matter with the environment. Production of metals, semiconductors and dielectrics – are open system. System may be in equilibrium and non-equilibrium states. The equilibrium state of system – unchangeable (constant) time system state. The constancy of state is not supported by the occurrence of any external to the process of system. Heterogeneous system – is a physicochemical system, within which there is an interface (or surface) that separating one from the other parts of the system in which occur abrupt change at least one of the system properties. Example: monocrystal in contact with the melt. Homogeneous system – a physical-chemical system within which no interface on which there would be abrupt change at least one of the properties of the system. Example: monocrystal, polycrystal. Substances which form the system called as components of the system. Components in the system presented in various phases. Phase – a homogenous system in equilibrium or set of homogeneous parts in heterogeneous system in equilibrium. In the other words, it is a homogeneous part of the system, limited from other parts of the system by interface, transferring through which the properties changes abruptly. Examples: 1) single phase system- quartz crystal. And also a lot of quartz crystals.
2) 2-phase system – a) crystal of Si, comprising the inclusion of SiO2; b) ice crystal in water and many ice crystals in water. The process of transition from liquid or gaseous state to solid, at the result of which forming the crystal lattice, and occur crystals called as crystallization. What explain the existence of liquid at one temperature, and at other temperatures of solid state and why the transformation occurs at well-defined temperatures? In nature, all spontaneously occurring conversions, and consequently crystallization and melting due to the fact that the new state in new conditions is energetically more stable, has lower energy content. We can say that the more free energy of the system, the system is less stable, and if it is possible, the system transferred into state where the free energy is less. For solids the most important feature of phase is its crystal lattice (atomic structure). Each phase has its own, only her inherent crystal lattice, which differs from the other phases by type or size of the unit cell. Allotropy and polymorphism – different structures of the same element with essentially same binding energy. Binding energy – the energy necessary for the separation of solid bodies into individual atoms, molecules or ions (depending on the composition of solid). Eb – binding energy is equal to the difference between the potential energies of isolated atoms and related systems, net of kinetic energy, which, according to the uncertainty principle, should be determined by the localization of nuclei and electrons of the outer shell. Different allotropic modifications of the same chemical element (α- and β- tin, α- and γ-iron, etc.) are different phases; phases are compounds, solid solutions on the basis of elements or compounds. In solid, you can specify three basic types of possible phases of the interaction of diverse components: 1) compounds; 2) solid solutions; 3) mechanical mixture. Compounds. Feature that this phase belong to chemical compounds, is the difference of the crystal lattice from lattice elements of which it is formed. 100
Solid solutions. Feature of the formation of solid solution is the conservation of the lattice-type component – solvent, but with different dimensions of the unit cell. In the result could form solution with limited and unlimited solubility with different temperature dependence of the solubility limit. On the basis of solvent (chemical element), there are 2 types of solid solutions: 1) substitutional solution – atoms of dissolved elements occupy the positions of solvent atoms in the lattice point (replaced them). Chem. el
а) б) Chem, compound
2) interstitial solution – atoms of dissolved elements occupy interstitial positions (interstices) in the lattice of solvent, penetrating between the atoms of the latter. In this case, the dimensions of soluble atoms must be smaller than the interstices. а)
3) omission solution- one of the components forming compound is present in amount exceeding definable relationship (as would be dissolved in the compound of stoichiometric composition), but it
takes in the lattice of compound inherent position and corresponding part of the position of another element remains unoccupied (vacant). Sb
- vacant positions
Stoichiometric compound (stoichiometric composition) – is chemical compound in which the valence of incoming component completely satisfied (no outstanding bondings). Mechanical mixtures are formed from two or more phases. Phase forming mixture can be elements or compounds. However, as rule, they are solid solutions. Forming of mechanical mixture occurs: 1) due to discharge of second phase from supersaturated solid solutions. 2) due to eutectic or eutectoid transformation. The eutectic (gr. Eutektos – easy melting): 1) granular mixture of solid solutions simultaneously crystallize from the melt at temperature lower than the melting temperature of individual components; 2) liquid melt or solution, from which such crystallisation is possible: eutectic transitions: 1) liquid phase s1 + s2 eutectoid transitions 2) s1 s2 + s3 Solid crystalline phase may be obtained as single crystals, polycrystals and amorphous solids, representing set of grains (or crystals). Differently oriented in space polycrystal crystallites are separated from each other by the interfaces – the grain boundaries – thickness of several interatomic distances. The grain boundaries are not the interphase boundaries in polycrystals. System components (К ) – chemical elements and compounds from which the phase can be constructed, that is, as the components may perform individual substances (chemical elements) or compounds. 102
Number of components (К) – minimum number of individual substances of which may be constructed any phase of the system. In general, the number of components can be less than the number of chemical elements contained in the composition of phase. Example: Compound of InAs and InP can form between each other continuous series of solid solutions: InAs – InP. Chemical elements – 3, components of the system -2- both compounds, as in any condition of alloy the total atomic percentage (As + P) = In. It should be noted that the physical-chemical system formed by the components is not adequate concepts. In the one-component systems are implemented phase, with constant chemical composition, which can be in various aggregate states as: solid, liquid and gaseous. The length of the existence region of particular phase or existence region of different phases of single-component system is determined by external parameters like temperature (T) and pressure (P). In the multi-phase systems are phases implemented as constants (individual substances) and, mainly, variables in chemical composition (solution) such phases are realized in solid, liquid or gaseous state. The length of the existence region of constant composition phase is determined by the values of the external parameters (P and T). The length of the existence regions of variable composition phase, as well as the region of different phase coexistence, defined as the values of the external parameters (P, T) and the composition of phases. Condensed systems – solids and liquids away from the critical point (the phase transition point). Solids and liquids are characterized by the compressibility of million times less than gas. Fundamental differences and character of the thermal motion of particles in condensed medium- is oscillating, in gases – forward. Depending on the temperature and pressure (for metals mainly on the temperature, P-sonst) all substances can be in four aggregate states: plasma, gaseous, liquid and solid. Plasma – an ionized gas, in which volume density of positive and negative electric charges are equal.
In gaseous state atoms are practically do not connected with each other and move randomly in space. In the liquid state atoms are poorly connected to each other, there is short-range order, the material takes the form of the vessel, parts are easily separable from each other. In the solid state atoms interact with each other by certain law, the structure has both short-range and long-range order, atoms form crystal lattice of species. The transition between aggregate states is accompanied by the change in free energy: F = U – TS
where U – internal energy; T – temperature; S=
q – entropy. T
There are 5 types of condensed systems: 1. liquid 2. glass 3. amorphous 4. liquid crystals 5. crystals Liquids – equilibrium, isotropic structurally disordered systems with fluidity, i.e., easily change its shape. Glass – quasi-equilibrium, isotropic structurally disordered systems with mechanical properties of solids. Amorphous – strongly non-equilibrium, isotropic, structurally disordered systems obtained under extreme conditions. Liquid crystals – equilibrium, anisotropic, partially structurally ordered systems with high fluidity. Crystals – equilibrium, anisotropic, structurally ordered systems (characterized by long-range order and translational symmetry). § 2. Phase equilibrium. The rule of phase. Gibbs Law In single-component or multi-component systems can be realized state, when in equilibrium are several phases. This condition is called heterogeneous equilibrium. Heterogeneous is equilibrium in system consisting of F-phase and K components realized under the following conditions: 104
К – lines
Т1=Т2=Т3=…=Тf Р1=Р2=Р3…=Рf µ11=µ12=µ13=…=µ1f µ21=µ22=µ23=…=µ2
(К+2) – lines
where the superscript К- is the number of components, the lower F – phase number, µкf –the chemical potential of the K- component in the F-phase. The concept of chemical potential is central in phase equilibrium. The system of equations (3.2) consists of (К+2) lines and F columns. In the first two lines contain the condition that temperature of each phase and pressure of each phase are the same throughout the system. The following K lines fixed position that the chemical potential µi of given component in all phases are same. Chemical potential of i-th component is called the work spent to increase the number of particles of the i-th grade at system to one unit at constant all the other variables that determine the thermodynamic potential (particle means atoms, molecules). Depending on the conditions in which phases, for describing used following thermodynamic potentials: G –isobaric-isothermal potential (Gibbs potential), F –free energy (Helmholtz energy) or isochoric-isothermal potential, U – internal energy of the system, H – enthalpy of the system (the heat of fusion, crystallization). G = H – TS или G = PV – TS,
where S – entropy. The chemical potential is a partial derivative of thermodynamic potentials by the number of particles of i-th component in phase:
G F H U N P ,T N T ,V N S , P N S ,V
where N – number of particles in single-component phase. In the analysis of heterogeneous equilibrium is important to know how many phases are in equilibrium, and how much number of system parameters can change independently without affecting number of phases in equilibrium. The answer to this question is given by the law, opened in 1876 by Gibbs and known as "phase rule". As the system parameters in one-component systems are the temperature (Т) and pressure (Р), in multicomponent systems – Т, Р and the concentration of the components in each phase – Х. In each phase consisting of К- components, the number of variables of concentration equal to: К 1 , so how
1 . Example: the
two-component system ХА+ ХВ=1, ХА= 1–ХВ. Such external parameters such as the characteristics of fields in which there are phases in the analysis of physical and chemical equilibria are usually not included in the assumption that they remain constant. The number of freedom degree or variation of the system- C – number of system parameters that can be changed without changing the number of phases in equilibrium. The value C is equal to the number of independent variables; i.e. minimum number of variables, which are selected and uniquely sets the other parameters. Thus, the value of C is equal to the difference between the total number of variables of system and the number of equations. The total number of variables in the system (3.2): F (К–1)+2. Variation of the system consisting of K – components and F – phase when the external parameters are only P and T is equal to: С = [(К-1)F + 2] – [К (F – 1)] The phase rule (or Gibbs law) provides quantitative relationship between the freedom degree of the system and number of phases and components: 106
mathematical notation of phase rule or Gibbs law, where C – is the number of freedom degrees, i.e., the number of external (temperature and pressure) and internal (concentration) factors that can change without changing the number of phases; K – number of components in the system; F – the number of phases. In those cases where the number of external parameters is decreased to one unit (P = const and T = const), the phase rule is written as follows: C=K–F+1
In those cases where the number of external parameters is zero, i.e. the pressure P and temperature T – constant (Р = const and T = const), the phase rule is written: C=K–F (3.7) Example: If C = 0, then any changing in temperature causes change in the number of phases; if C = 1, it is possible changing of temperature without changing the number of phases. In the liquid state: F = 1 – one phase; K = 1 – one component (pure metal); C = 1 – 1 + 1 = 1 – you can change the temperature without changing the aggregate state. The freedom degree for the alloy at the time of crystallization: F = 2 – two phases (liquid +crystals); K = 1 – one component (pure metal); C = 1 – 2 + 1 = 0 – equilibrium at strictly definite temperature (Tm). The number of relationship equations between variables (the concentrations of the components in phase) is prepared based on the requirements of the same chemical potential of component in all phases of the system (in equilibrium), since the chemical potential of
component in phase depends on the concentration of the component. This dependence is expressed by the equation: µ=µ0+kТln(γХ)
where µо – chemical potential of component in the standard state (under normal conditions), γ – activity coefficient of the component in phase, k –Boltzmann constant, Х – the concentration of component in phase. Therefore, under conditions of phase equilibrium occurs equilibrium redistribution of components between the phases. Consider an example: in system consisting of 2 components (К=2), in two-phase equilibrium condition (F=2) for each of the components (e.g., for component 1) is realized equation:
11 = 21
1 1 01 + kTln( 11 Х 11 ) = 02 + kTln( 21 Х 21 )
11 Х 11 1 1 ] = ( 02 – 02 )/ kT 1 1 2Х2
1 1 02 01 x11 21 k0 = 1 1 exp x2 1 kT
x11 where k0 = 1 – equilibrium distribution coefficient. In this case, x2 the distribution coefficient of component 1 between phases 1 and 2
x11 (for example 1 – – the ratio of concentration in the phase 1 and x2 phase 2 of the component 1 (the ratio of the concentrations of component 1 in solid and liquid phase). Thus, the distribution of the components (more accurately distribution of components concentration) between the phases is characterized by equilibrium 108
distribution coefficient, the value of which is derived from the equations of bonding type (3.12). In general case, the number of bonding equations for heterogeneous equilibrium in multiphase system is obtained from к of lower lines of system (3.2) and it is equal to: К(F– 1). To analyze the phase equilibrium phase law usually used in the form of (3.5; 3.6; 3.7) depending on conditions, in which located system. § 3. Construction methods of phase equilibrium diagrams The phase equilibrium can be described by both analytically and graphically. For graphic description used equilibrium phase diagrams (EPD) or phase diagrams (PD), which are sometimes called diagram of the system state. EPD of single component system is geometric representation of phase states, which are realized in single component system under various external parameters. FID component system built in the pressure-temperature coordinate (Р – Т). EPD of multicomponent system (К>1) is geometric image of the phase states (equilibria and transformation phase), realized under various parameters in the result of components interaction of the system. EPD of multicomponent system built in the coordinates of Р – Т – Х, where Х –concentration of the component. Each point of EPD characterize the physico-chemical parameters of systems resulting from the interaction of the components making up the EPD. EPD can be 2-dimensional, 3- dimensional, etc. With using EPD for the given conditions can determine: 1) number of phases in the system; 2) relative amount of each phase; 3) composition of each phase and its nature (i.e., pure component, solution, compound etc.) 4) character of phase transformations. It will be appreciated that the EPD without special explanations does not provide information about atomic structure of phases and their crystal lattice. EPD can be considered as fully reliable only after
using X-ray structure analysis (XSA) deciphered the atomic structure of each phases in the system. The main method of constructing EPD – method of physical and chemical analysis, foundations of which were developed by academician N.S. Kurnakov (Kurnakov IGIC RAS). The basis of physical-chemical analysis is the study of functional relationship between the physical properties values and Т, Р, Х parameters. Knowledge of these relationships allows to set the physical-chemical nature of the phases and boundaries of their existence. Physical properties are determined from the dependence of f(T), f(P), f(Х). Experimental methods used to build the EPD. 1. Thermographical analysis (differential-thermal analysis – DTA). 2. X-ray microanalysis. 3. X-ray structure (X-ray-graphical) analysis (XSA, XGA). It is also used electron microscopy (EM) and neutron radiography (NR). 4. Dilatometric analysis (measurement of density), and others. The essence of thermographical (DTA) and dilatometric methods of construction of EPD is that to the alloy with such composition temperature of phase transformation (the "critical points") determined by abrupt change in enthalpy H (H – melting heat) or volume (V) of the system on dependences Т = f (t) – time or Т = f(V) in the process of cooling or heating alloy. I.e. identify the critical points for the series of alloys, and then build all diagram. These methods are determined by the phase transitions of I-kind, as in any other phase transformations of thermodynamic potentials (G, F, H) changing without jump, because at equilibrium transformation temperature their values for old and new phases are equal. Phase transitions. Phase transitions can be I-st and II-nd kind. To first order phase transitions include transitions in which G, F, H thermodynamic potentials are changed without jump, but abruptly changed at the phase transition temperature of the first (partial) derivatives from thermodynamic potentials (at this case majority of transformations is allotropic (melting, etc.))
G T (G=H-TS=PV–TS): H; 1 T G S T P
G V ; P T (3.13)
That is first kind phase transitions that accompanied by abrupt changing in enthalpy (Н), volume (V) and entropy (S). Phase transitions of II-nd kind In some rarer phase transitions from one state to another: ferromagnetic paramagnetic; superconducting non-superconducting; ordered disordered. The first derivatives changed continuously, but changed abruptly the second derivatives of thermodynamic potentials.
2 G T H c p ; V V ; P T 1 2 P T Т P cP S T T P
where β – compressibility coefficient, (for solids cP ≈ cV). Phase transformations, accompanied by abrupt changing in the second derivatives of thermodynamic potentials are called phase transitions of II-nd kind. At phase transitions of the second kind first derivatives of thermodynamic potentials change continuously, but abruptly changed the second derivatives.
A common method of physical-chemical analysis is building diagram of "structure – property". For this composition we can build such diagram: Temperature – property; Pressure – property. As shown by N.S. Kurnakov and confirmed by huge factual material, based on geometric analysis of diagrams "structure – property" (or, in general case, " variable factor – property") existed two general principles: 1) principle of continuity 2) principle of conformity. According to the principle of continuity: at continuous change in the chemical composition (or other variable factors – Т, Р), is not accompanied by changing in the phase composition (number of phases), continuously and smoothly changing of system properties. According to the conformity principle, each phase and each phase equilibrium corresponds definite geometric image of the phase equilibrium diagram (EPD). The conformity principle more "capacious" principle, than the principle of continuity. As part of the conformity principle can also be formulated important provisions, which facilitate the analysis of phase diagrams: 1. All lines of double diagrams and surface of triple diagrams limited phase region, the number of phases which differ to one unit. 2. All sloped lines (surface) is characterized limited concentration of the primary dopant in the phase. The slope of line (surface) characterizes the temperature dependence of the concentration limits. 3. Dimensionality of geometric elements that characterize particular phase equilibrium responsible to variance (C) corresponding to the phase equilibrium. Example: points on the diagram characterize phase compositions undergoing monovariant transformation. 4. For alloy of any composition intersection of its with ordinate (y) lines (surfaces) in the diagram during the cooling or heating process is accompanied by changing of phase composition. In Table 3.1. specified properties of materials commonly used in the construction of the EPD. To obtain reliable conclusions about the structure of EPD should study not one, but also combination of several physical properties. 112
An important method for determining the number of phases (F) and their amount (concentration) is metallographic analysis. Table 3.1. Properties of materials most commonly used in the construction of phase equilibria diagrams Class of used properties Thermal
Electrical Magnetic Volumetric Force of bondings
Quantity that characterize property Heat of the phase transition Heat of formation Heat capacity Electrical resistivity Thermoelectric power Magnetic permeability Density Coefficient of thermal expansion hardness (microhardness)
Unit of measurement J/mol ----------J/(kg·К) Ohm·sm mV/К ----------g/sm3 К-1 MPa
In the analysis of the EPD (state diagrams) are primarily used Gibbs phase rule (C-variance of system, or the number of freedom degrees, K – the number of components): С = К – F + 2. a) If С = 0 – system is non-variant. The system can only exist under constant conditions. Change at least one of the parameters of system will cause change in the number of coexisting in equilibrium phases (F). b) If С = 1 – system is multivariant (singlevariant). However, only one parameter can be changed without changing the number of simultaneous equilibrium phases, etc. c) If С = 2 – divariant system (dualvariant). Two parameters can be changed without changing the number of simultaneous equilibrium phases. Example: Task: Consider the crystallization of silicon (Si) at Р=const from its liquid melt, heated to 1500оС. ТmSi = 1412oC. Determine the value of С for different phase regions. Solution: The number of external independent variables – (temperature) is equal to – 1, the number of components – 1. Upon
cooling the melt from 1500o С to 1412o С system is single-phase. Then С=К-F+1=1-1+1=1, that is temperatures in this range can be changed without changing the number of phases. Upon reaching Т=1412o С appears second (hard) phase, wherein С=К-F+1=1-2+1=0, that is, while there will be two phases, the system is non-variant. And the temperature will not fall until all liquid melt crystallized. This means that with the continued smooth decreasing of heater temperature in the physical-chemical system, the temperature will be maintained through the provision of the crystallization heat. In graph of Т=f(τ) will be T=const area, whose length is equal to the time from beginning to end of crystallization (τ-time).
What keeps the system temperature of Т=1412o С in conditions where the heat is continuously given to environment? The source of maintaining the temperature is released crystallization heat. In the case of transition of substance from one phase state to another is released into the external environment or absorbed from them additional amount of energy. This energy is called the heat of phase transition and is equal to the difference between the enthalpy of old and new phases. Task. Consider crystallization of germanium (Ge) at Р=const from its liquid melt, heated to 1200оС. Тm(Ge) = 940oC. Determine the value of С for the different phase regions.) 114
One should distinguish four possible cases of phase transitions (transformations): 1. During the transition from solid to liquid or vice versa generates heat melting or heat of crystallization: Solid phase liquid phase – heat of melting (crystallization) 2. During transition from one solid phase to another solid phase – generates heat recrystallization. Solid phase solid phase II – heat recrystallization 3. At the transition from solid state to gaseous state or vice versa generates heat of sublimation. Solid phase gas – heat of sublimation 4. During the transition from liquid to gaseous state, or vice versa released heat of evaporation. Liquid phase gas – heat of evaporation For the case of 1, 3, 4 – characterized by significantly greater absolute values of thermal effects, compared with the case 2. In Table 3.2. shown the values of the heat of melting for some elements. Table 3.2. The values of the heat of melting for some elements Elem ent Fe W C Si
Нm, kJ/mol 15,50 35,28 138,27 49,86
Eleme nt Ge Te Se S
Нm, kJ/mol 37,08 17,70 6,70 ± 1,68 1,72
§ 4. T – X diagrams of phase equilibrium of binary systems with unlimited solubility of the components Т–Х state diagrams of binary systems built in the coordinates of the temperature (Т) –concentration (Х). The concentration usually lay in atomic percentage (at.%) and sometimes used percent by weight. For systems in which one component is semiconductor (chemical element or compound), together with the diagrams constructed in
conventional scale, also built diagrams in which in the region adjacent to semiconductor, the concentration of doping component in at.% applied on logarithmic scale (Figure 3.1 в.), or build separate part of the diagram, adjacent to the semiconductor component, putting the concentration of 2nd component in atoms per cubic centimeter also in logarithmic scale (Figure 3.1. a). This is because the carrier concentration in semiconductor is measured in electrons (or holes) per cubic centimeter, and in those cases where dopants are providers of charge carriers, it is comfortable to measure carrier and impurity concentration in the same units. Furthermore, limit solubility of impurities in semiconductors, is generally very small ~(0,1– 0,01) % atm. and actually used doping concentration of (1014–1019) atoms/cm3, i.e., (106–10–1) % at. In these conditions it is important to show phase regions in the diagrams in which components concentration in the low concentration regions varies by one order of magnitude. The logarithmic scale used when in normal scale concentration range is less than 0.1% and merges with the ordinate axis.
Figure 3.1. – Т–Х phase equilibrium diagrams of two-component systems with limited solubility of component а – concentration in atoms per cubic centimeter; б – in atomic percent in linear scale; в – in atomic percentage; in the region adjacent to semiconductor, atomic percentages of dopant component plotted on logarithmic scale
Calculation of components concentrations from one scale to another (from at.% to % by weight) carried by the following formula: (3.15) Х 1 %(by weight ) / А1 100 Х %( аt.) [ Х 1 %(by weight ) / А1 ] [ Х 2 %(by weight ) / A2 ] 1
Х 1 %(by weight )
Х 1 %(аt.) А1 100 Х 1 % (аt.) А1 Х 2 %(аt.) А2
Хаt. / см 3
аtоm / см 3 100 N Х %(аt.) N 100
Где Х1 % (at.) – atomic percentages of 1 and 2 components Х2 % (at.) – percentages by weight of 1 and Х1 % (by weight) 2components Х2 % (by weight) А1 А2 3
– atomic masses of 1 and 2 components
Хat/sm3 – (usually write Хsm-3) number of impurity atoms in the 1 N – total number of atoms in the 1 sm3 N=
n , where n – number of atoms in the lattice, which are V
belong to one quantity of one unit cell; V – unit cell volume.
Task. Calculate the number of atoms per one unit cell quantity in the Bravais lattice. In the diagram of phase equilibrium (PED) represent phase regions separated from one of another by diagram lines (Figure 3.2).
Figure 3.2. – Typical phase equilibrium diagram of А–В binary system with unlimited solubility of components in the liquid (L) and solid (S) states. In the twophase region shown ab conode.
Any point on diagram can be viewed as figurative point of the alloy, describing its state. Projection of figurative point on the Х-axis indicates the composition (concentration) of alloy. Projection of the same point on axis Т – temperature axis at which this alloy is considered. Position of figurative point also indicates to the phase composition of alloy at this temperature. a and b points- figurative points of the phases, m pointfigurative point of alloy. If figurative point is in the single phase region, the phase composition matches with the alloy composition. If figurative point is within the two-phase region, the phases composition in equilibrium at given temperature is determined by conode passing through this point. Conode called a line segment, drawing at constant temperature (i.e., in isotherm) and enclosed within the two-phase region. Conode crosses the boundary of this region at points on the conjugate lines and figurative point phases which are in equilibrium at given temperature (a and b points), i.e. tie conode connecting points, characterized the composition of phases in 118
equilibrium (ab – conode). А' and В' points on EPD correspond to the melting temperature of the pure binary system of А and В components, respectively. А'аВ' line, above which all alloys is in liquid state is called the liquidus line (L): is the geometric locus of points characterizing the composition of liquid (L) phase (solution) of limiting concentration and temperature dependence of this concentration. А'bВ' below line in which all alloys in the solid state is called the solidus line (S): it is the geometric locus of points that characterize the composition of the solid (S) phase (solution) of limit concentration and temperature dependence of this concentration. The region between the solidus and liquidus lines – two-phase coexistence region of the liquid and solid phases (solution). The quantitative ratio of the phases in equilibrium at given temperature is determined by the lever rules: the ratio of the mass or volume amounts of Q-phases are in equilibrium at given temperature is inversely proportional to the ratio of conode segments, concluded between the figurative point of alloy and the figurative points of the respective phases. Example:
Figure 3.3. – Phase diagram with unlimited solubility of components in the solid and liquid states
At temperatures t1 alloy composition xm consists of two phases: liquid phase composition a (with concentration xa) and solid phase composition b (with concentration xb). The proportion of the phases equal to: QL(а) /QS(b) = mb/(ma)
Where QL(а) – composition of the liquid phase (Ха) QS(b) –solid phase composition in the (Хв) If you know the total mass or volume of alloy Qalloy, the absolute amount of liquid QL and solid QS phases determined from the following relationships: QL(а) = QALLOY mb /(ab)
QL(b) = QALLOY ma /(ab)
Task. To determine the variance of С system (Fig. 3.1) for: a) the pure А and В components at the melting temperature; б) alloys are in single phase regions (liquid and solid); в) alloys are in two phase region. Consider, as example crystallization of one from the real two component alloy system with unlimited solubility – Ge–Si alloy, containing 70% Si (Fig. 3.4).
Figure 3.4. – Phase diagram of Ge- Si system (а) and cooling curves of the alloy of 30% Ge + 70% Si (б) and pure germanium (в).
To t ≥t 1 temperature Х alloy composition is in the liquid solution state (L) and at cooling does not undergo phase transformations. Starting from t 1 temperature liquid solution is supersaturated with silicon and from liquid solution starts to separate solid solution α, where concentration of Si is larger than in original L, at the result melt is depleted by silicon. The first evolved α crystals have a composition corresponding to the figurative point a, i.e. 90% Si and 10% Ge. During cooling from t 1 to t 2 subsequent crystallization of the alloy occurs, during of which the amount of liquid phase is reduced, while solid increases. At t = t 3 disappear last drops of liquid melt. Proportion of liquid and solid phases coexisting at any given temperature is determined by the lever rule. Thus, at temperature t 2 QS/QL = (2 – с)/(2 – b)
Furthermore, during the crystallization from t 1 to t 3 changed the composition of the liquid and solid phases. If the process occur with very slow velocity- so that all conversions completed in time in accordance with the phase diagram, the liquid phase composition varies over the liquidus line from point 1 to point d, and the solid composition- on the solidus line from point а to point 3, as indicated by arrows. Both phases – disappears during crystallization, and the resulting – enriched during crystallization of the same component in the present case – Ge (germanium). This simultaneous enrichment of one and the same component is due to sharp decrease in number of simultaneous phase richer in this component (in this case, the liquid phase richer with germanium). Note that after the crystallisation process, passed under equilibrium conditions, there is only the solid phase, wherein its composition corresponds to the composition of the liquid solution (in the example is solid solution containing 70% Si). Conditions of EPD realization with unlimited solubility. А – В dual systems, A and B components which are infinitely dissolved in each other in the liquid and solid states, may be formed by chemical
elements and compounds. At the same time, both components must be: a) have the same type of chemical bonding; b) have the same type of crystal lattices; c) unit cell parameters (or atomic radius) should not differ (Δa, ΔR) than at (10-15)%; d) have similar potential relief of the crystal lattices of component. Such solutions are isovalent (with the same valence) substitution solutions (Table. 3.3) Table 3.3. Dual system (metal and semiconductor) with unlimited solubility of the components Solid solutions
Components Au-Cu Ag-Cu Au-Pd Ni-Cu Fe-Cr Mb-W
Structure FCC FCC FCC FCC BCC BCC
Δa or ΔR, % 11,2 11,3 5,0 3,0 9,9 9,9
V-Ti Ti-Mo Ge-Si InAs-InP GaAs-GaSb GaAs-GaP GaAs-InAs Bi2Te3-Bi2Se3 Bi2Te3-Sb2Te3
BCC BCC Diamond Blende Blende Blende Blende Tetradymite Tetradymite
2,0 5,0 10,4 3,2 8,0 3,0 8,0 8,0 8,0
From elementary diamond-like semiconductors equilibrium phase diagram with unlimited solubility form only silicon and germanium. They fully meet the requirements listed above. Silicon and carbon (diamond) meet the requirements of chemical nature and type of lattice, but differ greatly on the size of tetrahedral covalent radii (RSi = 0,117 nm, RC = 0,077 nm; ΔR/RSi = 36%). In this connection, the solubility of carbon in silicon is not more than one hundredth of percent, and silicon in carbon is less. Task. Define FCC, BCC, diamond lattice, sphalerite, tetradymite. 122
Application of solid solutions with unlimited solubility. Unlimited solubility – is very common feature among semiconductor compounds. They form together so many classes of AIIIВV, AIIBVI, A2VB3VI and etc. compounds (See. Table. 3.3). Such solid solutions are widely used. This is facilitated by the fact that solid solutions of semiconductors, with unlimited solubility allows to obtain alloys with any values of bandgap, lattice period (interatomic distances), coefficients of thermal expansion and number of other parameters in the range between their values for initial components. Periods of lattice changes in the first approximation, additively (Vegard's rule), other parameters – by more complex laws. Solid solutions with unlimited solubility (metallic or semiconductor) are widely used: 1. Au-Cu, Ag-Cu – in contacts of devices; 2. Cu-Ni – in electro-vacuum devices; 3. Fe-Cr – in stainless steel alloys (vacuum systems, etc.); 4. Mb-W, Mb-Ti, V-Ti – refractory materials; 5. Semiconductor semiconductor solid solutions – thermoelements, microelectronics, optoelectronics. Considering the opportunities created by solid solution with unlimited solubility, establishing the dependence of their properties on the composition is an important task of material science. § 5. Construction and analysis of diagrams with unlimited solubility according to the data about change of the thermodynamic potential. Coefficient of distribution As we know from thermodynamics, at constant temperature and constant pressure, that phase will be in equilibrium, for which observed isobaric-isothermal potential G = H – TS. H = U + PV и G = U + PV – TS In particular, for solid phase: U = U0 + UТ + UE, where U0 – potential energy of the lattice at T = 0 K; UТ –the energy of atoms thermal vibrations at given temperature; UЕ –elastic energy of the lattice distortion due to dissolution of foreign atoms; Р –external pressure; V – volume occupied by phase; S – entropy; T – the absolute temperature; N – phase enthalpy. Note that in general case,
the equilibrium state of the system is determined by the minimum of thermodynamic potential (G, U, H or F), which describes its state upon selected variable parameters. Entropy is always positive (S> 0) and increases with increasing temperature, so the temperature increases G decreases (Fig. 3.5 а); The curve G(T) is always facing upward convexity.
Figure 3.5. – Dependence of the isobaric-isothermal potential for liquid and solid phases of constant composition from temperature (а) and composition (б) for the liquid and solid phases of variable composition at Т=const, in which in equilibrium state is the solid phase
If we compare the temperature dependence of G for two phases (liquid and solid Fig. 3.5), then the slope of curves will always be different because of the difference S, so that the curves must intersect. The slope of G = f(T) will be steeper in that phase, in which S is greater. Entropy of liquid phase is greater than the entropy of solid phase of the same composition, however the curve for liquid phase is reduced more sharply than in solid. The point of intersection Тeq corresponds to the temperature of the phase transformation. Below and above this temperature are stable different phases respectively having smaller value of G. Consider the concentration dependence of G in the system formed by А and В components. In the ideal case, when А and В components do not dissolve into each other, any alloy of this system is mechanical mixture of А and В components and 124
dG / dX BA В tg
thermodynamic potential of any system alloy is found by additivity rule. If component B is soluble in component A, then until composition corresponding to the concentration limit (ХВsat), the dependence of G to concentration will be represented by continuous curve which is convex downwards, that is the equilibrium dissolution is associated with decreasing in G value of the solution. Consider the shape of curve G f ( X B ) near the component A (Fig. 3.5 б), e. g. in very dilute solutions region. A In this area dG / dX B is equal to the tangent angle between the tangent to the curve G=f(X) and the axis X and hence chemical A
potential of component B in solution concentration Х B : For ideal solutions
В Во RT ln X B
where Во –chemical potential of 1 mole В pure component (the value which depends only on the nature of component В); R – universal gas constant, equal to kNA, where k –Boltzmann constant, NA –Avogadro's number, so
dG / dX BA В Во RT ln X B
For infinitely dilute solutions ХВ → 0 and respectively ln ХВ → – ∞ and tgα → – ∞. This means that the curve G=f(XB) touched axis of ordinates, but it is especially important that at low concentrations of the A
components В in the derivative dG / dX B is always negative. Therefore, if impurity is dissolved in pure component, it is accompanied by decreasing in the isobaric-isothermal potential of the solution. This means that in these cases the process must always proceed in the direction of contamination of the pure component.
This conclusion is important for the processes of producing highpurity metallic, semiconducting and dielectric materials and emphasizes the need to minimize the almost inevitable pollution of environment, crucible material, and etc. Note that in all known experimental studies it was found that there is always at least tiny solubility of the components in each other. Thermodynamic characteristics of solutions. The length of the region of solution existence (both solid and liquid) is determined by number of its characteristics, including thermodynamic characteristics. Enter these specifications for two-component solutions. Most of the thermodynamic functions of the solution can be prepared by adding an additive thermodynamic functions of the components forming the solution. In particular, solution is formed only in the case when injected into solvent-additive decrease the isobaric-isothermal potential of solvent. Consider thermodynamic functions of 1 mole solution in its general form (index α –functions relating to the solution, о –functions relating to the pure components)
G X AG Ao X B GBo Gсм ;
S X A S Ao X Bo S Bo S см ;
H X A H Ao X B H Bo H см ;
V X AV Ao X BVBo Vсм where the index α – labeled solution, index 0 – component G , G Ao , G Bo – isobaric-isothermal potential of solution and А and В components; Gсм – isobaric-isothermal potential shifting of the solution; ХА and ХВ – concentration of А and В components in the solution;
S , S Ao , S Bo – entropy of solution and А and В compo-
nents; Sshift – entropy of solution shifting; H , H Ao , H Bo – enthalpy of solution and А and В components; Н см – enthalpy of
solution shifting; V ,V Ao ,VBo – volumes of the solution and А and В pure components; Vсм – volume of solution shifting. Based on the 1st and the 2nd law of thermodynamics can be shown that 126
Gсм H см TS см
If the description of thermodynamic functions of the solution to take into account only pairwise interactions between neighboring atoms, it can be shown that ΔНshift and ΔSshift equal to the following values:
H см Х А Х В АВ Sсм R( X А ln Х А Х В ln X B )
where ΩАВ –interaction parameter between А and В components in solution. (In the general case ΩАВ depends on the concentration of components and temperature. In those cases where ΩАВ practically constant magnitude of ΔНshift of solution depends on the concentration of ХА and ХВ). In turn, the interaction parameter is equal to:
ZN AB [ H AB ( H AA H BB ) / 2]
where Z – average coordination number in the solution, НАВ, НАА and НВВ – А−В, А−А and В−В enthalpy bondings. Task. Determine the average coordination number -Z for twocomponent solution consisting of 40% of component A and 60% of the component − В, if the valence of component A is equal to 3, and component В – 2. Depending on the structure and size of thermodynamic functions of shifting, as well as the coefficient of activity may be highlighted number of solutions types. Let us dwell on the consideration of only two types of solutions: ideal and regular. The approximation of these types of solutions can be described by many metal and semiconductor solutions, both in solid and in liquid state. However, it should take into account the limitations of the ideal models and regular solutions in the first place because they take into account
only the interaction between nearest neighbors. In Table 3.4. shown thermodynamic characteristics of the ideal and regular solutions. From the value of these characteristics should be the definition of these types of solutions. In general case, Gсм , ΔНshift, ΔSshift, Vсм –consider the interaction between atoms in the solution. Table 3.4. Thermodynamic characteristics of solutions Thermodynami c characteristic ∆Vshift ∆Hshift ∆Sshift ∆Gshift аА (concentration) аВ (concentration) γA (coefficient of activity А) γB (coefficient of activity В)
The value of thermodynamic characteristic for: Ideal solution regular solution 0 ≠0 0 (Ω=0) XAXBΩAB - R (XA lnXA – XB lnXB) - R (XA lnXA – XB lnXB) XAXBΩAB+ RТ (XA lnXA + RТ (XA lnXA – XB lnXB) XB lnXB) XA exp [ΩAB(1- XA)2/(RT )] XA XB
XB exp [ΩAB(1- XB)2/(RT)]
exp ΩAB(1- XA)2/RT
exp ΩAB(1- XB)2/RT
For ideal solution (mechanical mixture, there is no interaction between the components A and B) Vсм = 0, ΔНshift = 0, Н0 and V0 are additive that is determined by simple addition of the component; for the regular solution (B soluble in A, there is interaction A with B, and Ω ≠ 0) Vсм ≠ 0, ΔНshift≠ 0 Н0 and V0 are not additive (enthalpy changing, shifting different kinds of atoms). From thermodynamics follows that the formation of ideal solution under standard conditions is accompanied by changing in the isobaric-isothermal potential of shifting:
G см RT ( X
where – ХА and ХВ – concentration of components – A and B in solution. In the case of equilibrium coexistence of two ideal solutions (liquid and solid), based on the reference standard state (ТmА > ТmВ) changing of ΔGshift separately for each of the solutions of the form: G смLi Х
G m А RT ( X
So G см Х
G mB RT ( X
At the same time it is known that during the phase transition
G H TS
For pure component at its melting point (T=Tm) thermodynamic potentials of the liquid and solid phases are equal to: Т ТmА GmА ( Н Li Н So ) Т m ( S Li S So ) Н m Т m S m 0
From which for pure component
H m Т m S m ;
S m Н m / Т m .
At temperature different from Tm,
G mТ А ТmА Н m Т m S m 0 . Given the dependence of H m Т m S m and neglecting small temperature dependence H m and
S m the replacement ratio
Н m / Т m , is obtained for each of the components at T ≠ Tm, respectively: GmА Н mА (1 Т / Т mА );
G mВ Н mВ (1 Т / Т mВ ).
At equilibrium (coexistence) of the liquid and solid phase chemical potential μ for each component is the same both in liquid and in solid solution:
АSo АLi ВSo ВLi i.e. following relations is rightly: So Li d G см / dX АSo d G cм / dX ALi
So Li dGсм / dX ВSo dGcм / dX ВLi
Carry out further calculations relatively to the component B. Differentiating equations (3.32) and (3.33) and taking into account that ХА = 1 – ХВ, we get, respectively: Li G см G mА RT ( ln X ALi ln X ВLi ); dХ В
G So G mВ RT (ln X ВSo ln X АSo ); dХ В
Replacing GmА and GmВ by their values from (3.35) and (3.36) and equating the right side to (3.37) and (3.38), we obtain: Т
X B So Х АSo Н mА ln R Х ВLi Х АLi
1 1 Н mВ R T TmА
Consider alloys near pure component А, i.e. 130
1 1 T TmВ (3.39)
Х АSo 1, Х АLi 1, а 1 / Т 1 / Т mА , under such conditions the value
Х АSo Н mА 1 1 0 ln Li 0 and R T Т mА ХА Hence, we obtain
X BSo Н mВ ln Li R ХВ
1 1 T TmВ
Repeating similar arguments for the diagram region near to component В, we get
X АSo Н mА 1 1 ln Li R T TmА ХА
The equation of liquidus line for equilibrium with α-solid solution at low concentrations of component В, i.e. at Х АSo 1 has form
ln Х АLi ln 1 Х ВLi
Н mА 1 1 R Т mА Т
In the case of the formation of regular liquid solutions, equation (3.42) is transformed into
ln а АLi
Н mА 1 1 R Т mА Т
The calculation of liquidus and solidus lines in the Ge-Si system, conducted with the help of expressions (3.40) and (3.41), gives good agreement between the calculated and experimental data. This indirectly proves that germanium and silicon is formed between each other practically close to ideal liquid and solid solutions. In other cases, no such correspondence. The farther from the ideal solution, the greater the difference between calculated and experimental data. Thus, expression (3.40) and (3.41) can be used only in first approximation, in systems with unlimited solubility of components. If liquid solution is ideal, and solid solution is regular (i.e. enthalpy change in the case of different kinds of atoms shifting in the So 0 ), the expressions (3.40) and (3.41) are solid solution Н см converted to the form:
Н mВ S mВ So X So 1 Х ВSo ln BLi АВ ХВ RТ R RT
So X АSo Н mА S mА So АВ 1 Х А RТ R RT Х АLi
In the most general form of solutions for regular expressions (3.44) and (3.45) is converted into the equation of the form:
So LiAB 1 Х iLi XiSo Нmi Smi So АВ 1 Х i ln li Хi RТ R RT RT
where H mi and S mi – entropy and enthalpy of component melting, ratio of the concentrations in the solid and liquid phases considered in the left side of the equation; Х iLi and Х iSo – the concentration of i – component in the liquid and solid phases, respectively. However, using equation (3.46) for the construction of the solidus and liquidus lines is not always possible due to lack of the 132
thermodynamic characteristics of the solutions and their temperature and concentration dependence. They are usually only known for limited number of systems. Therefore, most often the problem is solved in the reverse order: the experimental phase diagrams build on the status of the liquidus and solidus lines in these diagrams determine the thermodynamic characteristics of the system. Building EPD with unlimited solubility according to the change of the thermodynamic potential. To construct the equilibrium phase diagrams of binary systems, in which it is known that the interaction of the components leads to the formation of continuous series of solid and liquid solutions, and are known melting temperature of the pure components ( Т Ао and Т Во ) and their temperature dependence G (Т) are fed as follows: 1) for several temperatures lying in the range between the melting temperatures of components ( Т Ао < Т i < Т Во ), construct isothermal curves showing concentration dependence of the isobaricisothermal potential of solid and liquid phases (Fig. 3.6. а, б);
а) temperature dependence G for A and B pure components in solid and liquid states,
Т А0 , Т В0 melting temperatures of A and B components
б) dependence of G for liquid and solid phases of variable composition at constant temperature Т1 (ХВl and ХВs –composition of liquid and solid phases in equilibrium at Т=Т1)
в) solidus and liquidus curves Figure 3.6. – Scheme of building solidus and liquidus curves from data on the temperature dependence G of pure А and В components in the solid and liquid phase (a), concentration dependence G of the solid and liquid phases in the case of binary system with unlimited solubility of the components in the solid and liquid states (a); б) the temperature dependence G of the pure A and B components in the solid and liquid states (
– composition of liquid and solid phases,
which are in equilibrium at Т1 )
2) through the graphical differentiation of these curves find coordinates of figurative points lying at selected temperature at the liquidus and solidus curves, corresponding to the compositions of the liquid and solid phases in equilibrium. The coordinates of figurative points are based on the fact that the values of the chemical potentials of the components at these points are equal to: µS = µL; or
G so Х so ; li Gli (Fig. 3.6. б), Х li
3) upon receipt figurative points build liquidus and solidus curves (Fig. 3.6. в). 4) find the points lying on the solidus and liquidus curves at Т=Т1. Find these points for other temperatures. 134
Distribution coefficient. The ratio of Х iSo / Х iLi in (3.45) and (3.46) expressions is an important characteristic of the equilibrium between solid and liquid phases (crystal – melt). This ratio of the concentration of the solute in the solid in the liquid phase at the same temperature, called distribution coefficient:
xiso k0 = li , at constant temperature xi From the diagram of phase equilibrium can be found values of equilibrium distribution of coefficients. However, since the solidus and liquidus lines are generally curvilinear, distribution coefficient k0 depends on the Xi concentration: k0 =f (Xi) For approximate estimating of values k0 liquidus and solidus lines usually replaced by tangent near the main component (solvent), as shown in Fig. 3.7. In this case, the value of k0 at low concentrations can be considered independent of the concentration of k0 f (Xi). As follows from Fig. 3.7., coefficient k0 > 1 corresponds to the case when the impurity increases the melting temperature of the solvent. At k0 < 1 melting temperature of the solvent decreases with impurities dissolved therein.
Figure 3.7. – Position of the liquidus and solidus lines near the component – solvent for cases k0 > 1 and k0 < 1.
Knowing the values of distribution coefficients is necessary to develop modes of metals and semiconductor materials treatment by zone melting: the more different from one k0, the more effective the treatment. From elementary diamond-like semiconductors (Ge, Si, C) diagram of phase equilibrium with unlimited solubility form only Ge and Si. They fully meet the above requirements. Si and C (diamond) meet the requirements of the chemical bonding (nature) and the type of lattice, but differ greatly on the size of tetrahedral covalent radii: RSi=0,117 nm, Rc=0,077 nm,
R 36% » (10÷15)% RSi
Therefore, the solubility of C in the Si is less than percent, and Si in C even less. Unlimited solubility – is very common phenomena among semiconductor compounds. They form a lot of connections between classes: АIIIBV, АIIBVI, АIVBVI, АIIIBV АVBVI and others. Such solid solutions are widely used. This is facilitated by the fact that solid solutions of semiconductors with unlimited solubility allows to obtain alloys with any values of bandgap, lattice period (interatomic distances), coefficients of thermal expansion and number of other parameters. The lattice period, in first approximation changed additively (Vegard rule), other parameters – for more complex laws. Given the opportunities created by such solid solutions, establishing the dependence of their properties on the composition is important task of material science. Tasks: 3.1. Determine the melting entropy of S m for Fe, W, Si, Te and compare obtained values with the character of changes in chemical bondings of these materials during the melting (melting temperature of Fe, W, Si and Te 1530, 3416, 1412, and 450 оС, respectively). 3.2. Ge contains the same concentration of background (harmful) impurity Cu (koCu = 1,5·10-5) and Sn (koSn = 2·10-2). Before obtaining from such material of perfect single crystal by the Czochralski method (from liquid solution-molten) it is subjected to zone melting for decreasing the concentration of Cu and Sn by several orders of 136
magnitude. Which of impurities requires fewer passes of zone melting? 3.3. How to change the value of distribution coefficient of impurities (if k0 < 1 and k0 > 1) by increasing the rate of crystal growth due to increased supercooling of the melt. 3.4. Water (ice) is formed with unknown impurity solution with unlimited solubility of the components in the liquid and solid state. This impurity increases the melting point of ice. At certain temperature Т system is in two-phase state (S + L). At one of the phases of the impurity concentration is less than at this Т? 3.5. Water with impurity is carried on frost. Half of water froze. Where impurities will be more: in the unfrozen water or ice? Consider the task for two cases: 1) k0 > 1 (impurity increases the temperature of melting ice); 2) k0 < 1 (impurity decrases the melting temperature of ice). § 6. T – X – diagrams of phase equilibrium of binary systems with unlimited solubility of the components Unlimited solubility of the components in each other is relatively rare, more often occur their interaction is complex. Within one binary system in different ranges of concentration can be realized (and often realized) different phases, which leads to complication of the phase equilibrium diagrams. Transition from unlimited solubility to limited. Thermodynamic analysis provides qualitative and in many cases quantitatively explain the transition from diagram with unlimited solubility to other types of phase diagrams. The starting point for deciding on the outcome of different kinds atoms interaction in their shifting is sign of the isobaric-isothermal potential of shifting:
Gсм H см T S см The amount of Gсм difficult depends on several factors, the main ones are two: 1) chemical, taking into account the degree of chemical affinity of the components (their valence, electronegativity, lattice type);
2) geometrical, taking into account the difference in the "atomic sizes" interacting components during the formation of solution: В where R R A RB / R A - the atomic radii of А and components, defined by chemical bonding occurring during the formation of solution. Increasing of components chemical affinity reduces the internal energy of the phase U , and therefore enthalpy value, as
H U PV U 0 U T U E PV
however in this case H см must be negative. Increasing the difference in the sizes of interacting atoms R should cause increasing in the internal energy U and enthalpy H , respectively, including the case of solid solution by increasing elastic deformation energy of the lattice ( U E ); thus it must be positive. It is necessary to distinguish the cases of chemical interaction in the formation of solid solution between nearest-neighbor atoms of one species (А–А) or (В–В) and the interaction between nearestneighbor atoms of different types (А–В). The corresponding binding (enthalpy) energy and denoted by Н АА , Н ВВ and Н АВ . In the case of ideal solution binding energy of atoms pairs of different kinds will be equal to the average of binding energy of the pairs of atoms of one kind, that is
Н АВ 1 / 2Н АА Н ВВ
In this case, the enthalpy of shifting H см = 0, as well as the interaction parameter Ω = 0 (see. Table. 3.4). In the real solution H см 0 . The sign of the enthalpy of shifting depends on the sign of Ω. Size of H см , can be negative or positive. It should, however, take into account that the result of components interaction is determined by value H см only at low 138
temperatures: T→0. With increasing temperature, according to the expression (3.27) becomes significant part of ТS см derivative (the so-called entropy term). Diagrams of phase equilibria with eutectic transition. In binary systems, in which the crystalline structure of the components are different, and their dissolution in each other leading to decreasing of crystallization temperature, can occur eutectic* transformation. Diagram with eutectic is shown schematically in Fig. 3.8а. It consists of six phase regions: single-phase region of liquid solution L, two-phase regions liquid solution L+ α solid solution and liquid solution L+ β solid solution; single-phase regions of α and β primary solid solutions; two-phase region of coexistence of α + β solid solutions. Slope of А'е and В'е liquidus line represent the geometrical place of figurative points of liquid solutions with limit concentration at appropriate temperatures. Slope of А'с and B'd solidus line is the geometrical place of figurative points of solid solutions with limit concentration that exist in certain temperatures above the eutectic temperature Te. The horizontal line ced- is a eutectic line. Only three points on the ced line are figurative, they characterize limiting concentration of solid solutions α (point с) and β (point d) and the liquid solution (point e) at temperature of eutectic transformation. * eutectic (eutektos – (greek) – easily meltable) – fine solids mixture simultaneously crystallize from the melt at temperature lower than the melting temperature of the individual components.
Figure 3.8. – Phase diagram of binary system with eutectic break of solubility: а –phase equilibria; б – cooling curve of alloys shown in the diagram; в –- isobaricisothermal potentials curves of liquid and solid phases at the eutectic temperature Те:
G GLi G Li . X B с Х В е1 X B d In Fig. 3.8в given the structure of isobaric-isothermal potentials curves of solid solutions α and β, and the liquid solution at the eutectic temperature. The eutectic temperature Т е and the position of eutectic points (e points) in the case of formation in the system of ideal liquid solutions and low solubility of the components in one another in the solid state can be calculated from the joint solution of the equations of liquidus components А and В: H A 1 1 exp R TA TE X A X B 1.
H B exp R
1 1 T T E B
Feature of ced eutectic line consists in that at the eutectic temperature (Те) in the composition of alloys from с to d in equilibrium are three phase of the above composition. Task. Determine the number of freedom degrees С in the alloys from с to d at Те. ас and bd sloping lines – geometric places of figurative points of limit concentration of solid solutions that exist at temperatures below the eutectic (solubility curves). During cooling of the single-phase region at line of intersection with the oblique line structure diagram of the alloy is in state saturated with the solution. Below the point of intersection begins disintegration of the supersaturated solution with the release of another phase, composition of which characterizes the point of intersection of conodes with the second oblique line bounding this two-phase region. Upon cooling within the two-phase region while changing the composition of two phases and their relative proportions.
The compositions of alloys from с to d occurs decay of liquid solution of the composition е to two solid solutions с and d cooling by the reaction: Lе↔Sс + Sd (cooling ↔ heating)
In the diagram in Fig. 3.8а shows the characteristic line of four alloys and corresponding cooling curves indicating the phase composition of alloys in different temperature ranges. The length of region on the cooling curve associated with invariant transformation of alloys Х3 and Хе, is proportional to the amount of liquid melt, turning into eutectic mixture at temperature Те. For alloy Хе this amount is 100%, and for alloys X 1 and Х 2 is 0% for others determined by the lever rule or law of additivity1. Note that when cooling any alloy, lying in the two-phase region α+β, starting from the temperature Те, changing the composition of both the solid solution on the curves са and db (thus they are depleted by dissolved component) and the quantitative ratio of the phases is determined according to the rule lever. For diagrams with eutectic is necessary to introduce, in addition to the concept of "phase", even the concept of "structural component". For diagram with unlimited solubility of these concepts are the same. In the α + β phase diagram with eutectic alloy phase composition for any alloy is the same – it is a mixture of phases α and β, but in terms of formation these phases, alloy differ by the nature of their location and form of particles. This distinction is important because the properties of alloys are dependent not only on the composition of phases but also on the geometry and nature of the particulate phase components of interposition. The structural components are primary crystals are released from the supersaturated liquid melt along the inclined lines (solidus) of diagrams; secondary crystals were released from the supersaturated solid solution along the inclined lines (lines of solubility) of the
Quantification comparison of the size of horizontal regions on curves of cooling or heating is possible only for alloys of identical mass.
diagram; eutectic (eutectic mixture), representing mixture of the crystals of two solid phases are simultaneously formed by the eutectic reaction (3.50). Schematic view of the various structural components2 shown in Fig. 3.9. Thus, alloys in the system shown in Fig. 3.8 а, comprise the following constituents: from А to Хα – α- primary crystals; from Хα to Хс – α- primary + β- secondary crystals; from Х с to Х е (hypoeutectic alloys) – α- primary crystals + eutectic (α + β)+ β- secondary crystals; Хе (eutectic alloy) – eutectic (α+β); from Хе to Хd (hypereutectic alloys) – β- primary crystals + eutectic (α+β) + α- secondary crystals; from Xd to Хb – β- primary + α- secondary crystals; from Хb to В – β- primary crystals. Diagrams with eutectic schematically described above are characterized by the fact that the maximum concentration of solutions α and β relatively large. Mutual solubility of the components, although limited, but is few to tens of percent. In these cases, the two components are elements with the same nature of chemical bondings.
When at eutectic transition temperature eutectic consists of primary crystals and in the case of decreasing temperature, appears the secondary crystals in it.
Figure 3.9. – Schematic image of some alloys structure of diagram with eutectic break solubility containing different structural components (а-д) and structure of the eutectic alloy quasibinary system of InTe-Sb2 (e) [alloy composition of 72% (mol.) Sb2 – 28% (mol). InTe; ×120]; and а – α-primary crystals; б – α-primary crystals + β-secondary crystals; в –α-primary «eutectic» (α + β); г –«eutectic» (α+β); д – βprimary crystal + eutectic.
Diagrams of phase equilibrium with degenerate eutectic transition. If one of the components of binary system semiconductor, i.e. has directed and saturated bondings and therefore poorly soluble in elements of different nature of bondings (great H см ), phase diagram changes. Metal-semiconductor phase diagrams are schematically shown in Fig. 3.10. Diagrams of the type shown in Fig. 3.10a, characteristic for systems Ag-Ge, Au-Ge, Al-Si. Diagrams of the type shown in Fig. 3. 10б, which called as diagram with degenerate eutectic (eutectic point close to the pure components) characterize the equilibrium in systems of In-Ge, Pb-Ge, Ga-Si, Zn-Si, Tl-Ge, Bi-Ge, Sn-Ge. Investigations carried out with the use of ultra-pure materials, the latest high-precision methods of structural analysis and measurement of electro-physical parameters have shown that there is always at least negligible mutual solubility of components. This confirms the validity of thermodynamic output, said earlier. Metals are dissolved in semiconductors, but in very small quantities that are calculated in hundredths and thousandths of atomic percent. 144
To display such low solubility in the phase diagrams is used, as mentioned above, the introduction of scale on the concentration axis. As an example is used phase diagrams image of Fe-Si and SiAu (in Fig. 3.1).
Figure 3.10. Phase diagrams of semiconductor-metal system with normal (а) and degenerate (б) eutectic.
The solubility of metals in semiconductors was not only small, but also dependent to temperature, which have great practical importance. As previously reviewed diagrams with eutectic maximum solubility of one component in the other occurred at the eutectic temperature Те. This regularity holds for most metal-based solutions. However, in the case of solutions based on semiconductors (Ge, Si, AIIIBV type compound) the maximum solubility is observed at temperatures well above the eutectic, and decreases towards the eutectic temperature Т е in several times. Thus, in the Si-Аu and SiFe systems (see. Fig. 3.1) solubility at Т е in 10 – 15 times lower than the maximum temperature (at Т > Те). This kind of dissolution, when it corresponds to the temperature exceeding the eutectic, called as retrograde solubility. Retrograde solubility is observed, for example, for solid solutions of metal in Ge, Si and АIIIBV semiconductors. In solid solutions of metal-based retrograde solubility is rare. Thermodynamic causes of retrograde solubility insufficiently studied. It is related to the large value of the shifting enthalpy by dissolving impurities in semiconductors.
Diagrams of phase equilibria with the eutectoid transformation. Transformations of eutectic type may experience not only liquid but also solid solutions. Non-variant transformation consists in the decomposition of the solid solution into two other solid phase, called the eutectoid, and the corresponding structural component – eutectoid. S1↔S2 + S3, (cooling ↔ heating)
A typical example of eutectoid transformation can serve transformation in the Fe-C system (Fig. 3.11).
Figure 3.11. The phase diagram of Fe-C system (а) and typical structure of the alloys of this system (б, в) after slow cooling (б – ferrite with carbon content of 0.6% (в – eutectoid steel).
In this system, austenite (solid solution of carbon in γ-iron with FCC lattice) containing 0.8% C, decomposes at 723 °C in mixture of two phases: Fе з С iron carbide (cementite) and solid solution of carbon in α-iron (BCC lattice) containing 0.04% C (ferrite): γ ↔ α + Fе з С, (cooling ↔ heating) Task. Determine the number of freedom degrees С at peretectoid transformation. Eutectoid structural component, comprising last two phases, called perlite. Number of perlite, shape and size of its constituent cementite particles have decisive effect on the properties of steel. This example well illustrates another important feature of the eutectoid transformation: it is associated with the movement (diffusion) of the components in solid solution at very long distance. Thus, to steel containing 0.8% C at eutectoid transformation produced FезС particles with the size of hundredth of micrometer (100 nm), carbon atoms have to collect from the 1.5 million unit cells. Character of diagrams with eutectic in semiconductor – metal systems plays an important role in the selection of alloys for doping of semiconductors and formation of contacts by fusing or melting – diffusion methods.
Diagrams of phase equilibria with peritectic transformation. One feature of the above diagrams with eutectic is that А and В components, dissolved in one another, decreasing melting temperature of solution both from A and from B. If, however, at limited solubility of components in each other one of them, for example В, dissolving in A, decreasing melting temperature of solutions based on it, as component A, dissolving in B, on the contrary, increases the Tm of solution instead of eutectic transition in diagram present as called peritectic transformation (n – peritectic point of transformation, Fig. 3.12 а). Eutectic transformation in binary system is the solution decay while cooling on the other two phases; peritectic transformation, on the contrary, is process of forming single phase through the interaction of the two other phases, completely or partially disappears at this. This reaction is written as follows: (cooling ↔ heating) L + Sb1 ↔ Sb2 or L + α ↔ β
Peritectic transformation in binary system is non-variant. Compositions of three equilibrium phases, as in the eutectic line, determined by the intersection points of ab horizontal line of peritectic with slanted lines in the phase diagram (i.e. a, n, b points)
In Figure 3.12. б shown the cooling curves for the five alloys like Х n , Х1 , Х 2, Х3 , X 4, compositions of which are shown in Fig. 3.12 a. On cooling curves indicated phase composition of the alloys in different temperature ranges. 148
Task. To determine the variance of the system at temperature Тn, Fig. 3.12 a. The length of region on the cooling curves at Тn for Хn, Х1, Х2 alloys is proportional to the number3 of interacting liquid solution and solid phase (by phase number formed by the peritectic reduction at Тn). For Хn alloy these relative amounts to 100%, for the other alloys of the region extent using the right lever can determine the proportion of alloy undergoes peritectic transformation. For alloys which compositions lie in the range of from Ха to Хn, the amount of liquid phase at temperature Тn is not enough for occurring interaction with all solid phase. As result, after peritectic transformation besides the new phase, alloys will contain an excess amount of primary crystals of α phase. For X1 alloy at temperature just below Тn excess amount of crystals in the alloy equal to (Х 1n /аn)·100%. Similarly, for the alloys which compositions lie in the range of from Хn to Хb, the number of phases α at Тn is small compared with the amount of liquid phase. As result, upon completion of peritectic conversion in alloys remain excess amount of the liquid phase. In Х2 alloy its relative amount is (nX2/nb L)·100%. An important feature of peritectic systems is that when the crystallization temperature Тn is completed only part of alloy undergoing peritectic transformation. As can be seen from the diagram in Fig. 3.12 alloys in the range of from Хn to X crystallization completed below Тn in line nВ'. Liquidus line (beginning of crystallization) is the line А'bВ', and the solidus line – the line А'аnВ'. Line аС is called the solubility curve. Line аb – peritectic horizontal, in which lies а, n and b three figurative points, corresponding to the composition of phases undergoing non-variant transformation.
3 Quantitative comparison of the sizes of horizontal regions on cooling or heating curves is possible only for alloys of identical mass.
If transformation similar to peritectic occurs only involving of solid phases, it is called peritectoid. S1 + S2 ↔ S3 or α + β ↔ γ (cooling ↔ heating)
Diagrams of phase equilibria with chemical compounds. As noted before, in case of large negative quantity of shifting so , i.e. in the case of large chemical affinity of system heat H см components and their interaction leads to the formation of chemical compounds. On the phase equilibrium diagram of chemical compounds are represented by vertical lines (at high temperatures can be observed deviation from the vertical). Consider the features of the phase diagrams with chemical compounds. From this perspective, all compounds can be classified in two ways: 1) by the ratio of the compounds and liquid phase formed during the melting of this compound. Compounds for which these compositions are same, are called congruent melting or persistent. If compositions are not identical, the compounds are called incongruently melting or unstable; 2) ability to dissolve other components in itself, including components of the compound, or alternatively, the ability to form solid solutions on their basis. One phase region of solid solutions of the components in this compound called homogeneity region. There are compounds with wide range of homogeneity region, calculated in percents, and compounds with narrow homogeneity region, calculate decimals and less proportions of percents and are not detectable in the phase equilibrium diagram, constructed in the normal scale. Congruently melting compounds are formed in many systems with semiconductor phases: АIII–ВIII, AIII–BIV and others. The melting temperature of such compounds lies on the liquidus line and line itself is a curve with maximum, which in many cases corresponds to the compound composition (Fig. 3.13 a). (Congruence – latin, congruens (congruentis) proportionate, appropriate, matching; in geometry – proportionality, matching, 150
match. Homogeneous – greek, homogenes – composition). This system always contains normal or degenerate eutectic and can be divided into partial simple eutectic systems, where compounds act as components of these systems and, therefore, compound ordinate divided diagram for private diagrams: M = q+1, where M – number of partial diagrams, q – number of congruently melting compounds in the system. Thus, systems of In-As and Ga-As are divided into two simple eutectic, Gr-Si – to four, i.e. congruently melting compound acts as system component. Incongruent melting compounds (Fig. 3.13). Melting of this type compounds, for example Ga3Te4 (Fig. 3.13. а), occur as peritectic type of transformation during heating, i.e. solid phase is converted into two phases – liquid and solid, the compositions of which lie on both sides of the composition of starting compound. Thus, the melting temperature of compound is below the liquidus line, whereby the latter does not have maximum associated with the compound. If in the system in addition to incongruent melting, there is congruently melting compound, then in appropriate range of concentrations for the liquidus line will experience maximum, as in the case with Ga-Te (see. Fig. 3.13 а) in the case of compounds GaTe and Ga2Te3. Break state diagram with unstable compounds into simple diagrams, taking the compound as component of the system, it is impossible.
Figure 3.13. – Phase diagram of systems with stable and unstable chemical compounds: а – system of Ga-Te, which produces two stable (GaTe and Ga2Te3) and two unstable (Ga3Te4 and Ga2Te5) compounds; б, в – Si-C systems at pressure Р ≈100 (б) и Р~1 (в); in system formed stable compound of SiC. In the system of Ga-Te melting temperatures of 1121, 1057, 1085ºC corresponding to GaTe, Ga3Te4, Ga2Te3 compounds.
Compounds forming broad region of homogeneity. Compounds of this type are quite common in metal and semiconductor 152
systems (metal compounds such as interstitial phases, chalcogenides, and others). Among the compounds of this type identified two groups: daltonides and berthollides. Daltonides – compounds with broad homogeneity region – characterized by the fact that the formulaic composition of compound within the homogeneity region (Fig. 3.14 а, б, в); common to the diagrams with daltonide phases is the presence of singular point on the liquidus and solidus curves, the composition of which corresponds to daltonides and simple stoichiometric ratio of the components. In the diagram of structure – property to formulaic composition of compound corresponds extreme value of properties. Berthollides characterized by the fact that formulaic composition of the compound lies outside of homogeneity region (see. Fig. 3.14 г, д). This means that for compounds of bertollide type of formulaic composition does not exist. The alloy corresponding to the formula of compound consisted of two phases, one of which is solid solution based on compound. Isochoricisothermal potential of such two-phase mixture is less than isochoricisothermal potential of compound strictly formulaic composition. In structure – properties diagram within the compositions of the homogeneity region, properties change monotonically.
Figure 3.14. – Systems that are formed daltonide (а, б, в) and bertolide (г, д)
phases; а, б – АхВу and АkBp compounds are congruent melting daltonide phases; в – incongruent melting АmBn compound – daltonide phase; г – γ phase with open maximum (liquidus curve) – bertollide phase; д – γ phase with concealed maximum (liquidus curve) – bertollide phase. In Fig. a shaded region of homogeneity of АхВу compound, in Fig. б – АkBp compound.
Compounds which form the narrow region of homogeneity. These include the majority of semiconductor compounds which form narrow range of solid solutions with components in the composition of compounds. Thus, the region width ranges from ten (for example, in compounds of A2IIIB3VI type, so much for In 2Те3 from 59.5 to 60% Te) to hundredths (AIIBVI) and even to thousandths (АIIIВV) of atomic percent. Despite the small amount, solubility plays a critical role in formation of compound physical properties. Therefore, study of features of solid solutions arranged in narrow region of homogeneity (i.e. with an excess of А and В components), is important and experimentally difficult task. One of the features is that in very large number of cases on the basis of AIIIBV and АIIВVI compounds within the homogeneity region formed superposition of solid solutions, for example omission solid solution and interstitial solid solution. The second feature is that the maximum melting temperature is necessary in these cases, the compositions are somewhat different from the stoichiometric compound and get strictly stoichiometric composition is difficult. Such compounds are called compounds with shifted stoichiometry. However, during small deviation from the stoichiometric composition, the compound melts with open maximum, are considered (in first approximation) as congruently melting compound. § 7. Dual semiconductor and dielectric phases General classification of dual semiconductor compounds did not exist. The most rational classification is based on the union to one class of compounds having the same stoichiometric formula and formed from the elements arranged in same groups of the periodic table of elements. Elements located in the periodic table in subgroups with fewer sequence numbers are designated by the letter A, and in subgroups with larger sequence numbers marked b B. Designations of elements of АIIIBV type should not be confused with their position in the periodic table, in the subgroups. 154
For example, compounds of class АIIIBV: GaAs. GaP, InSb formed by elements arranged in III A and V subgroups of the periodic system and its constituent compounds in equivalent proportions. V VI А 2 B3 : B2Te3, Sb2Te3, As2 Se3 class of compounds formed by elements located in the V A and VI subgroups of the periodic system and includes in ratio of 2: 3. Thus, class formula is generalized stoichiometric formula compounds included in this class. Regularities of binary phase semiconductor formation. Double semiconductor phases are double semiconductor compounds and solid solutions based on them. Chemical bondings in these phases mixed with covalent component predominance. Most often it is covalently-ionic-metalic bonding. Less is covalently-ionic. Ionic component of the bonding due to the fact that double phase constructed of dissimilar atoms. It characterizes the probability of belonging electrons to one of atoms, forming the bonding; if this probability is
1 , ionic component is equal to zero. 2
Metallic component characterizes the degree of blur cloud of valence electrons, forming chemical bonding. In the case of elementary semiconductors generalized qualitative characteristic of chemical bonding in the subgroup is the serial number of element. In the case of binary compounds generalized quantitative characteristic of chemical bonding in the same class of compounds is the average atomic number of compound:
C i Z i C i
where Сi – number of atoms of i – component; Zi – serial number of i -component.
For example, Zср for GaAs is equal to 32: Zср GaAs = (31+33)/ 2 =32; Zср of sesquioxide indium telluride (In2Te3) Zср In2Te3= (2*49+3*52)/ 5 =50,8 Within the class of compounds there is correlation between the properties of compounds and their average atomic number. Dual semiconductor phases are formed when essentially in hybrid bondings: sp, sp2 , sp3, dsp, d2sp3 and others. The presence of mixed bondings leads to complex crystal structure phase. Description of formation structures by Pauling (1935 y). For description of some structures Pauling introduced the concept of chemical bondings resonance.
Figure 3.15. – Spatial configurations of bondings implemented by orbitals: a) sp; – diagonal linear configuration, Zk=2; б) sp2; – trigonal planar, Zk=3; в) sp3; tetrahedral, Zk=4; г) d23p3 – octahedral, Zk = 6; д) trigonal pyramidal, Zk = 3.
It was found that most of the studied binary semiconductor phase subject to the following empirical regularities: 1) In most dual semiconductor phases performed the relation of Mooseri-Pearson (Canadian scientists): (ne/na) +в =8
where ne – number of valence electrons per formula of the compound (or the number of electrons participating in the formation of bondings); na – number of element atoms- anion, IV – VII В subgroup element accounting for the formula of the compound; в – average number of chemical bondings between atoms of element – anion per atom of the anion; determination of в value requires knowledge of the crystal structure of compound. «–» anion (greek аnа – up) – negatively charged ion; «+» cation (greek каtа – down) – positively charged ion. Phase, for which Mooseri-Pearson rule is executed effectively completes the valence shell of element atom – anion to 8. Rule of Mooseri-Pearson is equivalent (octets) to the Hume-Rothery rule for elementary semiconductors. Hume-Rothery first show that the structure of covalent crystals of chemical elements belonging to different groups of the periodic system and satisfies the rule: Zk=8–N
where Zk – coordination number; N – number of group in which located element (N – equal to the valence of the element); Zk is equal to the number of atom’s covalent bondings. Covalent crystal structure determined by the Hume-Rothery rule and direction of bondings, which can be found from the analysis of the wavefunctions of valence electrons. Covalent bondings as opposed to metallic characterized by orientation and saturation. Hume-Rothery rule can be written as follows:
Nв + Zk = 8
where Nв – number of valence electrons of element (for elements subject to the Hume-Rothery rule, it coincide with the number of the periodic system); Zk – number of valence electrons "give" on the formation of the chemical bonding by atoms of the first coordination sphere. This entry Hume-Rothery rule emphasizes the role of short-range order in the formation of semiconductor structures. In Table 3.5 shown examples of calculations by Mooseri – Pearson rule. Table 3.5. Examples of calculations according to the Mooseri – Pearson rule Compound GaAs CdTe Mg2 Si Ga2Te3 SiC
Class АIIIBV АIIBVI АIIBIV АIIIBVI АIVBVI
8 8 8 24 8
1 1 1 3 2
в 0 0 0 0 4
8 8 8 8 8
2) Dual-phase semiconductor comprise elements of IVA – VIIIA subgroup of the periodic system. 3) Most of semiconductor phases of IVА – VIIА elements obeys to the normal valence law хА = у (8-в)
where A and B are respectively the valence of elements A and B in the Ах Ву compound. A and B components included in the compound by ratio Х:У. For example: InSв: АIn = 3; ВSв = 5; 1 * 3 = 1 * (8-5) 4) The difference between the electronegativities of ∆Х elements included in the dual semiconductor phase is usually not small. ∆Х characterizes the ability of atom in the crystal (molecule) to attract valence electrons. The amount of ∆Х is proportional to : ∆Х ~ , where ∆ = ЕА-В – (ЕА-А + ЕВ-В)/2 158
ЕА-А, ЕА-В, ЕВ-В – binding energy between A-A, A-B, B-B atoms. Physically, the magnitude of Δ is similar to the value of the interaction parameter Ω. If the binding energy expressed in electron volts per atom, then ∆Х =
Note that, in general case, with increasing ∆Х increases proportion of ionic component of the bonding. § 8. Deviations from equilibrium state. The phase equilibrium diagrams role in selecting the conditions of crystallization and thermal treatment Liquation. (Liquation- melting, smelting, in metallurgy – (segregation) – inhomogeneity of chemical composition of the alloys occurs at crystallization because the alloys unlike pure metals do not crystallize at the same temperature and in the temperature range). Discussed earlier phase transformations are in equilibrium at given temperature. That is, the rate of temperature change is so small that at any given temperature, time to make all atomic motion associated with the change in the chemical and phase composition, dictated by the particular phase equilibrium diagram. However, these atomic movements carried out by diffusion takes time, the duration of which depends primarily on the nature of diffusing element, environment, temperature, size and perfection of the crystals, and other factors. In real conditions time required to reach equilibrium state may be different; by seconds or even fractions of second to many hundreds of hours. This explains the fact that in practice rarely observed equilibrium phase state. Moreover, such conditions are attained with difficulty, the same rule will be deviations in varying degrees from the equilibrium state. The most common example of this deviation is the liquation, which consists in the fact that chemical composition of the volume of crystal (ingot), solidified the beginning of crystallization is different
from the volume composition, crystallized in the last turn. To eliminate liquation using extended high-temperature heating (homogenizing annealing), but it is not always achieves equilibriumalignment structure over the entire crystal (ingot). Apply special methods of crystallization to obtain crystals with uniform distribution of impurities. Let us consider liquation phenomenon on the example of solid solutions formation. Liquation due to the fact that in any temperature of crystallization solid phase differs in composition from the liquid. The degree of this difference is characterized by the distribution ratio. Under equilibrium conditions k0 = СS/СL. In Fig. 3.16 shown liquation on the example of alloy with k0 < 1. Consider continuous crystallization of alloy r with composition С0 while cooling within temperature range of crystallization. In accordance with phase diagram at the starting temperature of crystallization it should appear crystal composition a, at temperature Т1 – crystals with composition b, at T2 – with composition c and etc. Thus, with decreasing temperature layers are formed of solid phase enriched in impurity component B. In conditions of equilibrium crystallization solids content corresponding to each value of temperature should be the same over the whole volume, and not only in layers, which crystallized at given temperature.
Figure 3.16. – Sceme of liquidation in alloys systems with unlimited solubility of the components.
To comply these conditions it is necessary: a) in solid phase can travel diffusion alignment of composition layers of early and late crystallization; б) to have time to go through diffusion alignment in the liquid phase. The last requirement is due to the fact that during the crystallization at k0 < 1 layer of liquid melt, which adjacent to the crystal surface enriched by impurity, as it were "stripped" crystal into the melt, because СS < СL, while in real conditions or crystallization alloys with k0 < 1 the effective distribution coefficient (kef) more than equilibrium distribution coefficient (k0). In the real conditions diffusion alignment in the solid phase because of significant cooling rate never goes completely, and crystallization goes on the nonequilibrium solidus. If we accept that in liquid phase has time to go through the composition alignment, non-uniform composition of solid solution is characterized by average concentration, which lies to the right of the line of non-equilibrium solidus a's' – in our scheme on the dotted line of a's. Thus, when temperature Т 1 solids content instead of b' is the average between b' and a', and will correspond to the point f; at Т2 –respectively to k point, average between b' and c', and etc. In conditions of non-equilibrium crystallization change not only the position of the solidus curve, but also the position of the liquidus curve. Thus completion of crystallization will not occur when nonequilibrium solidus temperature Т2, and at temperature Т c , when the average composition of solid phase lying on a's line's, would be equal to С0. If you put on the diagram the actual end point of crystallization for alloys of different composition under specific cooling conditions, we obtain line, which is called non-equilibrium solidus for selected conditions (a's line in Fig. 3.16). Decreasing the temperature of crystallization ending by increasing the cooling rate leads to the fact that in the case of alloys which form continuous series of solid solutions, the crystallizing composition of the latter portions of melt is close to the composition of the second (low-melting) component B. As result, the non-equilibrium crystallization of crystal chemical composition of the cross section is non-uniform. If crystallization occur with large supercooling, i.e. at temperatures much lower than the equilibrium temperature of the onset of
crystallization, the solidification front is obtained is very uneven, crystals grow in the form of dendritic (tree-like formations). "Axes" of dendrites crystallizes first if they contain fewer impurities than the crystal region solidify last. This phenomenon is called the intracrystalline or dendritic liquation. Different chemical composition of the alloy causes different effects on chemical etching, which allows to good identify intracrystalline liquation using metallographic methods (Fig. 3.17).
Figure 3.17. – Microstructure of the alloy with traces of dendritic crystallization before (а) and after (б) annealing.
Above it was assumed that the alignment of liquid phase composition in the crystallization process go to completion. However, in practice and it is not possible to observe because of the following reasons. Aligning the melt composition is carried out primarily by diffusion. The effectiveness degree of this process depends on the rate of diffusion of impurities in the melt, cooling rate, and the distribution coefficient. Furthermore diffusion for composition alignment can create convection currents in the melt by stirring. However, in this case the travel speed of melt layer directly adjacent to the surface of solid phase is very small, and only way to the composition alignment structure in this layer is diffusion. As noted, among other factors on the effectiveness of melt composition equalization influences the cooling rate. With its increasing equalization process in liquid solution will be more suppressed. At very high speeds the cooling diffusion redistribution of different types atoms in the melt is not possible. Under these 162
conditions, the crystallizing composition of solid solution will be equal to the composition in liquid phase. This process is called diffusionless crystallization. Obtaining alloys by such method have practical interest. Deviations from equilibrium state, even more sharply than in systems with unlimited solubility, achieved in conditions of accelerated cooling systems with eutectic and peritectic transformations. Thus, in systems with eutectic alloys, single phase in equilibrium crystallization conditions may be two-phase in non-equilibrium crystallization conditions. The consequences of such non-equilibrium crystallization under favorable conditions, can be shot long leveling (homogenizing) annealing (Fig. 3.17 б). Metastable phases. EPD with metastable phases. Another important example of deviation from equilibrium is formation of metastable phases in the phase transitions process. So called non-equilibrium phase, which are in some cases: a) transitional stage between initial and equilibrium phase, in others б) phase stable at certain pressure, temperature and concentrations ratios. On the phase equilibrium diagram of metastable equilibrium depicted by dashed lines. Metastable phases formed by crystallization of elementary substances and binary alloys with considerable supercooling of the melt (solution), temperature and concentration range in which the phases are metastable, has different length. Isobaric-isothermal potential of the metastable phase is less than in original, but greater than in the equilibrium phase, so the transformation of the metastable phase to equilibrium requires certain activation energy, absence of which the metastable phase can exist indefinitely. Formation of metastable phases – phenomenon often observed and widely used and transformations in the solid state. This includes, above all, the formation of supersaturated solid solutions, if their decay is carried out at low temperatures, when the diffusion and thus the formation of the equilibrium phases difficult.
There is every reason to believe that observed in heavily doped semiconductors concentration mismatch of electrically active impurity and its overall (chemical) concentration (polytropic impurities) is in many cases the result of the initial stages of solid solution decomposition, in which the impurities are formed with the participation of metastable phases. Metastable phases are also formed in sharp cooling of solid solutions that have at equilibrium cooling experience eutectoid transformation. An illustration of this is the martensitic transformation during quenching of steel (austenite). Many of metastable states cause the alloys useful and sometimes unique properties. The aim of material science – establishment of the nature of these non-equilibrium states and development of the fundamental mode, which allows to obtain metastable state. The starting point for solving these problems is the knowledge of phase equilibria diagrams. For description of metastable phases using special equilibrium phase diagram of metastable phases – the so-called metastable diagrams. Region of the metastable and metastable chemical compounds on these diagrams shown by dashed line. The question about application of the phase rule to metastable diagrams is debatable. In Fig. 3.17 (2) shown the equilibrium phase diagram of Co-C and Ni-C systems and metastable diagrams of these systems. The value of metastability is determined by the difference between the energies of metastable phase and mixture of stable phases. At very high cooling rates (102 – 1010) K/s of supercooled melts (solutions) below certain temperature can be obtained solid metastable phase not only in crystalline but also in amorphous state (when phase has short-range order, and has not got long-range order in the arrangement of atoms). Alloys in amorphous state can be obtained not only during the crystallization from the liquid phase, but also during the deposition from the gaseous phase. For obtaining amorphous phases with covalent type of bonding requires lower cooling rate compared with the metallic bonding type of phases. Knowing the phase equilibrium diagram is also necessary in the case of choosing liquid phase composition and temperature conditions of crystallization. This is particularly important in the preparation of crystal compounds. Let's consider on the example of producing single crystals by pulling them from the liquid phase by Czochralski method. 164
Crystallization occurs at the seed-crystal, which in contact with the surface of molten liquid, supercooled to ΔT below the liquidus temperature. This supercooling is maintained throughout the crystallization process. As crystallization of solid phase new layers on seed crystal pulled from the liquid phase. The composition of crystallizing solid phase is determined by the phase equilibrium diagram, if in the process of drawing support conditions close to equilibrium (crystallization rate is small, wide spread diffusion processes in the solid and liquid phase, i.e. ∆Т→0).
Figure 3.17 (2). – Metastable diagrams (solid lines – stable, dashed lines – metastable equilibrium): а – possible metastable equilibrium in the diagram of eutectic type; б – possible metastable equilibrium in the diagram of peritectic type; в – metastable diagram of the Co-C system; г –metastable diagram of the Ni-C system.
Congruently melting compounds, e.g. GaTe and Ga2Te3 (see. Fig. 3.13 a) can be obtained from the liquid phase of the same composition as compound. They can be prepared by crystallization from the melt and slightly different composition: for example, compound GaTe – from melt composition Х1 crystallization at temperature in the range of between 1100 and 1019 K. However, it should be noted that if compound has certain homogeneity, then pulled crystal will not have stoichiometric composition, and will be solid solution with limit concentration based on the compound, the equilibrium temperature for crystallization. Incongruent melting compound can not be obtained from the liquid phase of the same composition. Thus, in Fig. 3.13 shown that from the liquid phase corresponding in composition to GaTe3 at supercooling below the liquidus line will crystallize Ga 2 Te 3 , solid phase composition, but not GaTe 3 . During the crystallization from the liquid phase allocated congruently melting compound GaTe3, liquid phase composition should lie in the range of concentrations from Х 2 to Х 3 , and crystallization should be carried out at temperature between Т 3 (~760 К) and Т 4 (709 К). Consideration of the above crystallization incongruent melting compound called as crystallization from solution. In contrast from this crystallization from the liquid phase corresponding to the composition of crystallizing solid phase, called the crystallization from the melt. In general, the concept of "melt" and "liquid solution" require clarification. Under melt should be understood liquid phase having composition on the main (primary) component (components) corresponding to the composition of elementary substance or compound within the accuracy of their determination, and contents of background impurities and dopants, which does not exceed (1 – 2)% (atom). Under liquid solution to be understood liquid phase, the composition of the main components of which does not coincide with the composition of solid phase, as well as liquid phase, the contents of background impurities and dopants which exceed (1 – 2)% (at.). § 9. P – T and P – T – X diagrams of phase equilibrium The use of high and ultra-high pressure (several tens of GPa) in number of cases leads to change in the type of phase diagram, dramatic shift of the phase transformation temperature, appearance of new phases 166
that are not in the system at atmospheric pressure. Importance of studying the phase equilibrium diagram, constructed in the Р – Т – X coordinates (where Р –external pressure) connected with this. Thus the basic regularity is difficult that pressure increasing impede to the conversion, connected with increase of the specific volume, and expands on the composition and temperature of the existence region of phases with high density. Due to the increased role in semiconductor electronics of various kinds of semiconductor compounds and solid solutions based on them, containing volatile components have interest to study the phase diagram, constructed in the р – Т – X coordinates, where p – vapor pressure of volatile component or pressure of its dissociation. In systems which components have low dissociation pressure, and in which the maximum melting temperature of mixture below the lowest boiling temperature of component, the role of gaseous phase can be neglected. Phase diagrams for these systems is typically built to temperatures below the boiling temperature. In Fig. 3.18 is given example of phase diagrams with eutectic at temperatures below the boiling point of pure components. If the dissociation pressure of any component is large, the composition of gaseous phase must be considered at temperatures both above and below the liquidus temperature substantially throughout the range of temperatures, which investigated the phase equilibria in the studied system. Thus, one should distinguish phase diagrams for systems with low pressure dissociation in which Р – external pressure affecting, in Figure 3.18. – Phase diagram of particular, on the phase transforsystem with eutectic gap of mation in the solid state, and for solubility and low pressure of systems with large dissociation components dissociation pressure, in which р – vapor pressure of volatile component or dissociation pressure; we denote it by рdis. The main feature of these phase diagrams is the appearance
of geometric elements that describe the composition of gaseous phase. Phase diagrams constructed in the P – T coordinates. Diagrams of single component system presented in the Р–Т coordinates are diagrams projection constructed in the G–Т–Р coordinates (where G –isobaric-isothermal potential) on the plane Р– Т (Fig. 3.19). G–Т–Р diagrams demonstrate the equality of chemical potentials of the component (or adequate to it in single-component system – isobaric-isothermal equality potential phase) under phase equilibrium. Р–Т diagrams are phase diagrams of one-component systems, in which the phase transformation caused only by changes in temperature and pressure. P-T diagrams of substances which do not undergo polymorphous transformation in the solid state, shown schematically in Fig. 3.19, б, в. The phase regions corresponding to solid, liquid and vapor state, separated by monovariant twophase equilibria lines: ОА –curve of sublimation; АС –melting curve; АВ –curve of evaporation (boiling), along with ongoing equality: GS = GL or GL = GV or μS = μV, μS = μL or μL = μV. Point A is non-variant and corresponds to the three-phase equilibrium. Task. Determine the number of freedom degrees at point A, Fig.3.19. The diagrams in Fig. 3.19, б, в, different slope of the melting curve AC. The slope of each of the two curves is determined by the sign of the derivative dТm/dP, which in turn is determined by the sign change in the specific volume of the phase transition type. Increasing the pressure increases temperature of phase transformation, if it is accompanied by increasing in the specific volume and decreases this temperature, if during the phase transformation process specific volume decreases.
Figure 3.19 – Phase diagram of one-component system: а – diagram built in G–T–P coordinates; said surface isobaric-isothermal potential G of the individual phases of the two lines of intersection of these surfaces meet monovariant, and the point of intersection of three surfaces – non-variant phase equilibrium; б, в – diagram constructed in Р – Т coordinates, while the melting of solid phase is accompanied by increasing ( б ) and decreasing (в) of specific volume
Thus, at dV/dT > 0 and dT/dP > 0 phase transformation line tilted to the right, and at dV/dT < 0 and dТ/dP < 0 – to the left. Evaporation and sublimation are always accompanied by increase in the specific volume, so the curves OA and AB are always inclined to the right. The sign change of specific volume and, hence, the density in the melting is ambiguous. If melting of metals ∆V is always positive (Fig. 3.19, б ), then in the case of melting semiconductors sign of change ∆V depends on whether the transition is accompanied by liquid state change in the nature of chemical bondings or not. Upon melting of semiconductors, the following two cases of transition from solid to liquid are possible: 1) semiconductor → semiconductor 2) semiconductor → metal. In the first case, typical of such substances as sulfur, selenium, tellurium, compounds of Bi2Te3, Cu2S, some compounds of АIIВVI type (e.g. CdTe), ∆V > 0, at the second characteristically for germanium and silicon, as well as for number of compounds of АIIIВV type, on the contrary, ΔV